# Electronic Supplementary Material (ESI) for CrystEngComm.
# This journal is © The Royal Society of Chemistry 2016

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_sb974_cu_hpw_vd_4_no_na_125k2_red_abs
_database_code_depnum_ccdc_archive 'CCDC 1420704'
_audit_update_record             
;
2015-08-26 deposited with the CCDC.
2016-05-19 downloaded from the CCDC.
;
_audit_creation_date             2015-06-19
_audit_creation_method           
;
Olex2 1.2
(compiled 2015.01.26 svn.r3151 for OlexSys, GUI svn.r4998)
;
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Cu0.5 O42.5 P W12, Cu O5, 4.75(O)'
_chemical_formula_sum            'Cu1.50 H24.50 O52.25 P W12'
_chemical_formula_weight         3193.17
_chemical_melting_point          ?
_chemical_oxdiff_formula         'Cu1.5 P W12 O51.5'
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/n 1'
_space_group_name_Hall           '-P 2yn'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'

_cell_length_a                   12.9417(2)
_cell_length_b                   21.8435(3)
_cell_length_c                   15.0559(2)
_cell_angle_alpha                90
_cell_angle_beta                 94.1800(13)
_cell_angle_gamma                90
_cell_volume                     4244.85(11)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    17019
_cell_measurement_temperature    123(1)
_cell_measurement_theta_max      28.7540
_cell_measurement_theta_min      1.8480
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    33.273
_exptl_absorpt_correction_T_max  0.050
_exptl_absorpt_correction_T_min  0.004
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details   
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
Analytical numeric absorption correction using a multifaceted crystal
			model based on expressions derived by R.C. Clark & J.S. Reid.
(Clark, R. C. & Reid, J. S. (1995). Acta Cryst. A51, 887-897)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            'light blue'
_exptl_crystal_colour_modifier   light
_exptl_crystal_colour_primary    blue
_exptl_crystal_density_diffrn    4.997
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       prism
_exptl_crystal_F_000             5556
_exptl_crystal_size_max          0.6557
_exptl_crystal_size_mid          0.3113
_exptl_crystal_size_min          0.1757
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0420
_diffrn_reflns_av_unetI/netI     0.0298
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.926
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       29
_diffrn_reflns_limit_k_min       -29
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            52136
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.926
_diffrn_reflns_theta_full        26.000
_diffrn_reflns_theta_max         28.989
_diffrn_reflns_theta_min         1.646
_diffrn_ambient_environment      N~2~
_diffrn_ambient_temperature      123(1)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 16.1183
_diffrn_detector_type            Eos
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.926
_diffrn_measurement_details      
;
#__ type_ start__ end____ width___ exp.time_
  1 omega  -36.00  -10.00   1.0000   14.0400
omega____ theta____ kappa____ phi______ frames
    -       27.3621  129.0000 -149.1181 26

#__ type_ start__ end____ width___ exp.time_
  2 omega -112.00  -45.00   1.0000   14.0400
omega____ theta____ kappa____ phi______ frames
    -      -28.1433  178.0000  120.0000 67

#__ type_ start__ end____ width___ exp.time_
  3 omega -108.00   12.00   1.0000   14.0400
omega____ theta____ kappa____ phi______ frames
    -      -28.1433  -77.0000   30.0000 120

#__ type_ start__ end____ width___ exp.time_
  4 omega  -38.00   46.00   1.0000   14.0400
omega____ theta____ kappa____ phi______ frames
    -      -28.1433   37.0000  -30.0000 84

#__ type_ start__ end____ width___ exp.time_
  5 omega   57.00   99.00   1.0000   14.0400
omega____ theta____ kappa____ phi______ frames
    -       27.3621  178.0000  120.0000 42

#__ type_ start__ end____ width___ exp.time_
  6 omega -102.00    7.00   1.0000   14.0400
omega____ theta____ kappa____ phi______ frames
    -      -28.1433  -57.0000   90.0000 109

#__ type_ start__ end____ width___ exp.time_
  7 omega  -49.00   52.00   1.0000   14.0400
omega____ theta____ kappa____ phi______ frames
    -      -28.1433   37.0000  150.0000 101

#__ type_ start__ end____ width___ exp.time_
  8 omega -119.00  -32.00   1.0000   14.0400
omega____ theta____ kappa____ phi______ frames
    -      -28.1433  178.0000  -30.0000 87

#__ type_ start__ end____ width___ exp.time_
  9 omega -108.00   22.00   1.0000   14.0400
omega____ theta____ kappa____ phi______ frames
    -      -28.1433  -37.0000 -180.0000 130
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Xcalibur, Eos, Gemini ultra'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_UB_11      0.0330340000
_diffrn_orient_matrix_UB_12      0.0098900000
_diffrn_orient_matrix_UB_13      -0.0327545000
_diffrn_orient_matrix_UB_21      0.0047911000
_diffrn_orient_matrix_UB_22      -0.0306567000
_diffrn_orient_matrix_UB_23      -0.0146856000
_diffrn_orient_matrix_UB_31      -0.0436663000
_diffrn_orient_matrix_UB_32      0.0041294000
_diffrn_orient_matrix_UB_33      -0.0306789000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   'Enhance (Mo) X-ray Source'
_diffrn_special_details          ?
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                9222
_reflns_number_total             10443
_reflns_odcompleteness_completeness 99.98
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     26.32
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_data_collection       
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_data_reduction        
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2008)'
_computing_structure_solution    'ShelXS (Sheldrick, 2008)'
_refine_diff_density_max         4.649
_refine_diff_density_min         -2.107
_refine_diff_density_rms         0.321
_refine_ls_extinction_coef       0.000073(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.167
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     656
_refine_ls_number_reflns         10443
_refine_ls_number_restraints     71
_refine_ls_R_factor_all          0.0360
_refine_ls_R_factor_gt           0.0291
_refine_ls_restrained_S_all      1.293
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0147P)²+69.2504P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0635
_refine_ls_wR_factor_ref         0.0656
_refine_special_details          ?
_olex2_refinement_description    
;
1. Restrained distances
 Cu2A-O46
 1.98 with sigma of 0.02
 Cu2A-O49A
 1.98 with sigma of 0.02
 Cu2A-O48A
 1.98 with sigma of 0.02
 Cu2A-O50A
 2.36 with sigma of 0.02
 Cu2A-O49B = Cu2A-O47A
 1.98 with sigma of 0.02
 Cu2B-O47B
 1.98 with sigma of 0.02
 Cu2B-O46
 1.98 with sigma of 0.02
 Cu2B-O49B
 1.98 with sigma of 0.001
 Cu2B-O48B
 1.98 with sigma of 0.02
 Cu2B-O50B
 2.36 with sigma of 0.02
2. Uiso/Uaniso restraints and constraints
Uanis(O52W) \\sim Ueq, Uanis(O51W) \\sim Ueq, Uanis(O53W) \\sim Ueq: with sigma
of 0.01 and sigma for terminal atoms of 0.02
Uanis(O48B) \\sim Ueq, Uanis(O48A) \\sim Ueq, Uanis(O46) \\sim Ueq, Uanis(O47B)
\\sim Ueq, Uanis(O47A) \\sim Ueq, Uanis(O49B) \\sim Ueq, Uanis(O49A) \\sim Ueq:
with sigma of 0.001 and sigma for terminal atoms of 0.002
Uanis(O50A) = Uanis(O50B)
Uanis(O48B) = Uanis(O48A) = Uanis(O49A) = Uanis(O47A) = Uanis(O46) =
Uanis(O49B) = Uanis(O47B)
3. Others
 Fixed Sof: Cu2A(0.25) Cu2B(0.25) O46(0.5) O47A(0.25) O47B(0.25) O48A(0.25)
 O48B(0.25) O49A(0.25) O49B(0.25) O50A(0.25) O50B(0.25) O51W(0.5) O52W(0.25)
 O53W(0.25) O57W(0.25) O58W(0.25) O59W(0.25)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.68241(3) 0.39683(2) 0.35608(2) 0.00946(7) Uani 1 1 d . . . . .
W2 W 0.61078(3) 0.40082(2) 0.58834(2) 0.00847(7) Uani 1 1 d . . . . .
W3 W 0.78553(3) 0.28013(2) 0.51645(2) 0.00896(7) Uani 1 1 d . . . . .
W4 W 0.69328(3) 0.16661(2) 0.37679(2) 0.01157(8) Uani 1 1 d . . . . .
W5 W 0.59203(3) 0.28265(2) 0.21645(2) 0.01084(7) Uani 1 1 d . . . . .
W6 W 0.42792(3) 0.39322(2) 0.27921(2) 0.01032(7) Uani 1 1 d . . . . .
W7 W 0.35754(3) 0.40089(2) 0.51169(2) 0.00783(7) Uani 1 1 d . . . . .
W8 W 0.44716(3) 0.29385(2) 0.66197(2) 0.00784(7) Uani 1 1 d . . . . .
W9 W 0.62443(3) 0.17252(2) 0.59217(2) 0.00871(7) Uani 1 1 d . . . . .
W10 W 0.41600(3) 0.16492(2) 0.29812(2) 0.00978(7) Uani 1 1 d . . . . .
W11 W 0.34807(3) 0.16975(2) 0.51351(2) 0.00884(7) Uani 1 1 d . . . . .
W12 W 0.25403(3) 0.27628(2) 0.36341(2) 0.00870(7) Uani 1 1 d . . . . .
Cu1 Cu 0.45601(8) 0.00656(5) 0.16540(7) 0.0117(2) Uani 1 1 d . . . . .
Cu2A Cu 0.3850(4) 0.5024(2) 0.0709(3) 0.0247(11) Uani 0.25 1 d D . P A 2
Cu2B Cu 0.4624(4) 0.5123(2) 0.1008(3) 0.0185(9) Uani 0.25 1 d D . P A 1
P1 P 0.51999(16) 0.28346(9) 0.43971(13) 0.0055(4) Uani 1 1 d . . . . .
O1 O 0.4954(4) 0.3260(2) 0.5164(4) 0.0059(11) Uani 1 1 d . . . . .
O2 O 0.5448(5) 0.3217(3) 0.3595(4) 0.0095(11) Uani 1 1 d . . . . .
O3 O 0.6141(5) 0.2436(3) 0.4684(4) 0.0091(11) Uani 1 1 d . . . . .
O4 O 0.4268(4) 0.2425(3) 0.4143(4) 0.0093(11) Uani 1 1 d . . . . .
O5 O 0.5524(5) 0.1457(3) 0.3461(4) 0.0139(13) Uani 1 1 d . . . . .
O6 O 0.3643(5) 0.1296(3) 0.4014(4) 0.0118(12) Uani 1 1 d . . . . .
O7 O 0.2914(5) 0.2119(3) 0.2860(4) 0.0113(12) Uani 1 1 d . . . . .
O8 O 0.4832(5) 0.2265(3) 0.2348(4) 0.0102(12) Uani 1 1 d . . . . .
O9 O 0.6752(5) 0.2277(3) 0.2874(4) 0.0122(12) Uani 1 1 d . . . . .
O10 O 0.4898(5) 0.3453(3) 0.1929(4) 0.0136(12) Uani 1 1 d . . . . .
O11 O 0.6872(5) 0.3463(3) 0.2517(4) 0.0118(12) Uani 1 1 d . . . . .
O12 O 0.7613(5) 0.3354(3) 0.4193(4) 0.0103(12) Uani 1 1 d . . . . .
O13 O 0.6386(5) 0.4193(3) 0.4683(4) 0.0104(12) Uani 1 1 d . . . . .
O14 O 0.5609(5) 0.4330(3) 0.3008(4) 0.0107(12) Uani 1 1 d . . . . .
O15 O 0.4001(5) 0.4171(3) 0.3969(4) 0.0103(12) Uani 1 1 d . . . . .
O16 O 0.3286(5) 0.3317(3) 0.2937(4) 0.0095(11) Uani 1 1 d . . . . .
O17 O 0.2807(4) 0.3345(3) 0.4563(4) 0.0103(12) Uani 1 1 d . . . . .
O18 O 0.2389(5) 0.2154(3) 0.4512(4) 0.0111(12) Uani 1 1 d . . . . .
O19 O 0.3644(5) 0.2346(3) 0.5964(4) 0.0099(11) Uani 1 1 d . . . . .
O20 O 0.4875(5) 0.1503(3) 0.5457(4) 0.0104(12) Uani 1 1 d . . . . .
O21 O 0.6776(5) 0.1319(3) 0.4917(4) 0.0126(12) Uani 1 1 d . . . . .
O22 O 0.7477(5) 0.2190(3) 0.5987(4) 0.0109(12) Uani 1 1 d . . . . .
O23 O 0.5572(5) 0.2371(3) 0.6490(4) 0.0097(11) Uani 1 1 d . . . . .
O24 O 0.5494(4) 0.3562(3) 0.6797(4) 0.0097(11) Uani 1 1 d . . . . .
O25 O 0.3525(5) 0.3557(3) 0.6203(4) 0.0106(12) Uani 1 1 d . . . . .
O26 O 0.4779(5) 0.4391(3) 0.5649(4) 0.0103(12) Uani 1 1 d . . . . .
O27 O 0.7097(5) 0.3380(3) 0.5804(4) 0.0105(12) Uani 1 1 d . . . . .
O28 O 0.8018(5) 0.2148(3) 0.4336(4) 0.0130(12) Uani 1 1 d . . . . .
O29 O 0.3933(5) 0.1076(3) 0.2230(4) 0.0166(13) Uani 1 1 d . . . . .
O30 O 0.6243(5) 0.2668(3) 0.1123(4) 0.0156(13) Uani 1 1 d . . . . .
O31 O 0.3629(5) 0.4466(3) 0.2149(4) 0.0165(13) Uani 1 1 d . . . . .
O32 O 0.1288(5) 0.2903(3) 0.3305(4) 0.0153(13) Uani 1 1 d . . . . .
O33 O 0.2639(5) 0.4542(3) 0.5225(4) 0.0121(12) Uani 1 1 d . . . . .
O34 O 0.6758(5) 0.4560(3) 0.6492(4) 0.0150(13) Uani 1 1 d . . . . .
O35 O 0.7722(5) 0.4508(3) 0.3366(4) 0.0143(13) Uani 1 1 d . . . . .
O36 O 0.9106(5) 0.2951(3) 0.5497(4) 0.0141(13) Uani 1 1 d . . . . .
O37 O 0.7600(5) 0.1111(3) 0.3273(4) 0.0191(14) Uani 1 1 d . . . . .
O38 O 0.2817(5) 0.1161(3) 0.5685(4) 0.0143(13) Uani 1 1 d . . . . .
O39 O 0.6486(5) 0.1207(3) 0.6747(4) 0.0138(13) Uani 1 1 d . . . . .
O40 O 0.4168(5) 0.2819(3) 0.7681(4) 0.0132(12) Uani 1 1 d . . . . .
O41 O 0.5229(6) -0.0274(4) 0.2773(5) 0.0305(18) Uani 1 1 d . . . . .
O42 O 0.5848(5) 0.0491(3) 0.1500(5) 0.0188(14) Uani 1 1 d . . . . .
O43 O 0.3844(5) 0.0360(3) 0.0531(4) 0.0118(12) Uani 1 1 d . . . . .
O44 O 0.3289(5) -0.0362(3) 0.1882(4) 0.0156(13) Uani 1 1 d . . . . .
O45 O 0.5103(5) -0.0785(3) 0.0846(4) 0.0159(13) Uani 1 1 d . . . . .
O46 O 0.3844(9) 0.5828(5) 0.1400(8) 0.0125(15) Uani 0.5 1 d D U P . .
O47A O 0.2278(13) 0.5049(11) 0.0571(16) 0.0125(15) Uani 0.25 1 d D U P A 2
O47B O 0.3488(16) 0.4781(11) 0.0256(15) 0.0125(15) Uani 0.25 1 d D U P A 1
O48A O 0.3745(19) 0.4195(8) 0.0184(15) 0.0125(15) Uani 0.25 1 d D U P A 2
O48B O 0.5555(19) 0.4448(10) 0.0714(16) 0.0125(15) Uani 0.25 1 d D U P A 1
O49A O 0.5339(13) 0.4866(11) 0.0806(16) 0.0125(15) Uani 0.25 1 d D U P A 2
O49B O 0.5527(15) 0.5398(10) 0.2048(10) 0.0125(15) Uani 0.25 1 d D U P A 1
O50A O 0.389(3) 0.5399(13) -0.0746(14) 0.029(5) Uani 0.25 1 d D . P A 2
O50B O 0.540(2) 0.5714(12) -0.0058(18) 0.029(5) Uani 0.25 1 d D . P A 1
O51W O 0.5740(17) 0.0160(8) 0.4440(10) 0.040(4) Uani 0.5 1 d . U P B 1
O52W O 0.497(3) 0.0202(16) 0.438(2) 0.037(8) Uani 0.25 1 d . U P C 2
O53W O 0.684(3) -0.0076(17) 0.352(3) 0.049(10) Uani 0.25 1 d . U P . .
O54W O 1.0188(8) 0.1669(5) 0.4544(10) 0.086(5) Uani 1 1 d . . . . .
O55W O 0.0950(5) 0.3542(3) 0.5457(5) 0.0182(14) Uani 1 1 d . . . . .
O56W O 0.4258(6) 0.1466(3) 0.7694(5) 0.0239(16) Uani 1 1 d . . . . .
O57W O 0.567(2) 0.5029(13) 0.1325(19) 0.024(6) Uiso 0.25 1 d . . P D 3
O58W O 0.285(2) 0.5075(14) 0.023(2) 0.027(7) Uiso 0.25 1 d . . P E 3
O59W O 0.155(2) 0.5023(14) 0.076(2) 0.028(7) Uiso 0.25 1 d . . P F 3


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O2 2.425(6) . ?
W1 O11 1.926(6) . ?
W1 O12 1.900(6) . ?
W1 O13 1.886(6) . ?
W1 O14 1.897(6) . ?
W1 O35 1.696(6) . ?
W2 O1 2.417(5) . ?
W2 O13 1.911(6) . ?
W2 O24 1.905(6) . ?
W2 O26 1.921(6) . ?
W2 O27 1.886(6) . ?
W2 O34 1.700(6) . ?
W3 O3 2.419(6) . ?
W3 O12 1.904(6) . ?
W3 O22 1.908(6) . ?
W3 O27 1.905(6) . ?
W3 O28 1.917(6) . ?
W3 O36 1.691(6) . ?
W4 O3 2.446(6) . ?
W4 O5 1.903(6) . ?
W4 O9 1.897(6) . ?
W4 O21 1.913(6) . ?
W4 O28 1.907(6) . ?
W4 O37 1.693(6) . ?
W5 O2 2.436(6) . ?
W5 O8 1.903(6) . ?
W5 O9 1.891(6) . ?
W5 O10 1.919(6) . ?
W5 O11 1.906(6) . ?
W5 O30 1.687(6) . ?
W6 O2 2.433(6) . ?
W6 O10 1.891(6) . ?
W6 O14 1.934(6) . ?
W6 O15 1.907(6) . ?
W6 O16 1.883(6) . ?
W6 O31 1.699(6) . ?
W7 O1 2.418(5) . ?
W7 O15 1.885(6) . ?
W7 O17 1.915(6) . ?
W7 O25 1.914(6) . ?
W7 O26 1.892(6) . ?
W7 O33 1.697(6) . ?
W8 O1 2.426(5) . ?
W8 O19 1.908(6) . ?
W8 O23 1.909(6) . ?
W8 O24 1.905(6) . ?
W8 O25 1.900(6) . ?
W8 O40 1.693(6) . ?
W9 O3 2.422(6) . ?
W9 O20 1.919(6) . ?
W9 O21 1.924(6) . ?
W9 O22 1.888(6) . ?
W9 O23 1.894(6) . ?
W9 O39 1.693(6) . ?
W10 O4 2.431(6) . ?
W10 O5 1.905(6) . ?
W10 O6 1.902(6) . ?
W10 O7 1.908(6) . ?
W10 O8 1.896(6) . ?
W10 O29 1.698(6) . ?
W11 O4 2.452(6) . ?
W11 O6 1.927(6) . ?
W11 O18 1.917(6) . ?
W11 O19 1.890(6) . ?
W11 O20 1.883(6) . ?
W11 O38 1.703(6) . ?
W12 O4 2.425(6) . ?
W12 O7 1.911(6) . ?
W12 O16 1.909(6) . ?
W12 O17 1.903(6) . ?
W12 O18 1.896(6) . ?
W12 O32 1.688(6) . ?
Cu1 O41 1.982(7) . ?
Cu1 O42 1.937(7) . ?
Cu1 O43 1.976(6) . ?
Cu1 O44 1.944(6) . ?
Cu1 O45 2.357(6) . ?
Cu2A O31 2.523(8) . ?
Cu2A O46 2.040(10) . ?
Cu2A O47A 2.031(16) . ?
Cu2A O48A 1.976(16) . ?
Cu2A O49A 1.952(16) . ?
Cu2A O50A 2.343(17) . ?
Cu2B O31 2.645(8) . ?
Cu2B O46 1.955(10) . ?
Cu2B O47B 1.938(16) . ?
Cu2B O48B 1.975(16) . ?
Cu2B O49B 1.9779(10) . ?
Cu2B O50B 2.343(17) . ?
P1 O1 1.534(6) . ?
P1 O2 1.522(6) . ?
P1 O3 1.534(6) . ?
P1 O4 1.529(6) . ?
O48B O50B 1.57(4) 3_665 ?
O49A O50A 1.16(4) 3_665 ?
O50A O49A 1.16(4) 3_665 ?
O50B Cu2B 2.32(3) 3_665 ?
O50B O48B 1.57(4) 3_665 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O11 W1 O2 72.3(2) . . ?
O12 W1 O2 83.1(2) . . ?
O12 W1 O11 87.5(2) . . ?
O13 W1 O2 83.5(2) . . ?
O13 W1 O11 155.5(2) . . ?
O13 W1 O12 85.4(3) . . ?
O13 W1 O14 89.5(3) . . ?
O14 W1 O2 72.8(2) . . ?
O14 W1 O11 87.5(3) . . ?
O14 W1 O12 155.8(2) . . ?
O35 W1 O2 171.0(2) . . ?
O35 W1 O11 101.2(3) . . ?
O35 W1 O12 103.2(3) . . ?
O35 W1 O13 103.3(3) . . ?
O35 W1 O14 101.0(3) . . ?
O13 W2 O1 82.6(2) . . ?
O13 W2 O26 87.9(3) . . ?
O24 W2 O1 72.6(2) . . ?
O24 W2 O13 155.2(2) . . ?
O24 W2 O26 86.6(2) . . ?
O26 W2 O1 72.3(2) . . ?
O27 W2 O1 83.1(2) . . ?
O27 W2 O13 85.3(3) . . ?
O27 W2 O24 89.7(3) . . ?
O27 W2 O26 155.1(2) . . ?
O34 W2 O1 170.8(3) . . ?
O34 W2 O13 103.9(3) . . ?
O34 W2 O24 100.9(3) . . ?
O34 W2 O26 101.1(3) . . ?
O34 W2 O27 103.8(3) . . ?
O12 W3 O3 83.3(2) . . ?
O12 W3 O22 154.9(3) . . ?
O12 W3 O27 84.6(2) . . ?
O12 W3 O28 89.5(2) . . ?
O22 W3 O3 71.9(2) . . ?
O22 W3 O28 87.0(3) . . ?
O27 W3 O3 82.8(2) . . ?
O27 W3 O22 88.3(2) . . ?
O27 W3 O28 155.3(3) . . ?
O28 W3 O3 72.6(2) . . ?
O36 W3 O3 171.8(2) . . ?
O36 W3 O12 101.8(3) . . ?
O36 W3 O22 103.2(3) . . ?
O36 W3 O27 103.8(3) . . ?
O36 W3 O28 100.9(3) . . ?
O5 W4 O3 82.5(2) . . ?
O5 W4 O21 87.8(3) . . ?
O5 W4 O28 154.5(3) . . ?
O9 W4 O3 83.2(2) . . ?
O9 W4 O5 86.0(3) . . ?
O9 W4 O21 154.7(3) . . ?
O9 W4 O28 88.8(3) . . ?
O21 W4 O3 71.7(2) . . ?
O28 W4 O3 72.1(2) . . ?
O28 W4 O21 86.4(3) . . ?
O37 W4 O3 171.3(3) . . ?
O37 W4 O5 103.4(3) . . ?
O37 W4 O9 103.4(3) . . ?
O37 W4 O21 101.8(3) . . ?
O37 W4 O28 102.1(3) . . ?
O8 W5 O2 82.0(2) . . ?
O8 W5 O10 88.8(3) . . ?
O8 W5 O11 154.1(2) . . ?
O9 W5 O2 83.8(2) . . ?
O9 W5 O8 84.6(3) . . ?
O9 W5 O10 156.1(3) . . ?
O9 W5 O11 88.6(2) . . ?
O10 W5 O2 72.5(2) . . ?
O11 W5 O2 72.4(2) . . ?
O11 W5 O10 87.4(3) . . ?
O30 W5 O2 171.3(3) . . ?
O30 W5 O8 103.8(3) . . ?
O30 W5 O9 103.0(3) . . ?
O30 W5 O10 100.9(3) . . ?
O30 W5 O11 102.1(3) . . ?
O10 W6 O2 73.0(2) . . ?
O10 W6 O14 87.0(3) . . ?
O10 W6 O15 155.2(2) . . ?
O14 W6 O2 72.0(2) . . ?
O15 W6 O2 82.3(2) . . ?
O15 W6 O14 87.0(3) . . ?
O16 W6 O2 83.6(2) . . ?
O16 W6 O10 90.6(3) . . ?
O16 W6 O14 155.2(2) . . ?
O16 W6 O15 84.9(2) . . ?
O31 W6 O2 171.0(3) . . ?
O31 W6 O10 101.9(3) . . ?
O31 W6 O14 100.7(3) . . ?
O31 W6 O15 102.8(3) . . ?
O31 W6 O16 104.0(3) . . ?
O15 W7 O1 83.7(2) . . ?
O15 W7 O17 85.4(2) . . ?
O15 W7 O25 155.5(2) . . ?
O15 W7 O26 91.1(3) . . ?
O17 W7 O1 81.9(2) . . ?
O25 W7 O1 72.4(2) . . ?
O25 W7 O17 86.1(2) . . ?
O26 W7 O1 72.7(2) . . ?
O26 W7 O17 154.6(2) . . ?
O26 W7 O25 86.7(3) . . ?
O33 W7 O1 172.8(2) . . ?
O33 W7 O15 102.5(3) . . ?
O33 W7 O17 102.1(3) . . ?
O33 W7 O25 101.7(3) . . ?
O33 W7 O26 103.2(3) . . ?
O19 W8 O1 84.3(2) . . ?
O19 W8 O23 84.3(2) . . ?
O23 W8 O1 81.6(2) . . ?
O24 W8 O1 72.4(2) . . ?
O24 W8 O19 156.3(2) . . ?
O24 W8 O23 87.9(2) . . ?
O25 W8 O1 72.4(2) . . ?
O25 W8 O19 89.3(2) . . ?
O25 W8 O23 153.7(2) . . ?
O25 W8 O24 87.8(2) . . ?
O40 W8 O1 171.8(2) . . ?
O40 W8 O19 102.9(3) . . ?
O40 W8 O23 102.9(3) . . ?
O40 W8 O24 100.6(3) . . ?
O40 W8 O25 103.5(3) . . ?
O20 W9 O3 83.3(2) . . ?
O20 W9 O21 88.3(3) . . ?
O21 W9 O3 72.1(2) . . ?
O22 W9 O3 72.2(2) . . ?
O22 W9 O20 155.4(2) . . ?
O22 W9 O21 86.5(3) . . ?
O22 W9 O23 89.4(3) . . ?
O23 W9 O3 82.5(2) . . ?
O23 W9 O20 84.9(3) . . ?
O23 W9 O21 154.3(2) . . ?
O39 W9 O3 172.0(3) . . ?
O39 W9 O20 102.4(3) . . ?
O39 W9 O21 102.2(3) . . ?
O39 W9 O22 102.2(3) . . ?
O39 W9 O23 103.5(3) . . ?
O5 W10 O4 83.0(2) . . ?
O5 W10 O7 155.2(2) . . ?
O6 W10 O4 72.5(2) . . ?
O6 W10 O5 88.4(3) . . ?
O6 W10 O7 87.2(3) . . ?
O7 W10 O4 72.4(2) . . ?
O8 W10 O4 82.1(2) . . ?
O8 W10 O5 84.3(3) . . ?
O8 W10 O6 154.3(2) . . ?
O8 W10 O7 89.2(3) . . ?
O29 W10 O4 172.2(3) . . ?
O29 W10 O5 101.5(3) . . ?
O29 W10 O6 101.1(3) . . ?
O29 W10 O7 103.2(3) . . ?
O29 W10 O8 104.5(3) . . ?
O6 W11 O4 71.6(2) . . ?
O18 W11 O4 71.9(2) . . ?
O18 W11 O6 86.1(3) . . ?
O19 W11 O4 83.4(2) . . ?
O19 W11 O6 154.9(3) . . ?
O19 W11 O18 88.6(2) . . ?
O20 W11 O4 82.5(2) . . ?
O20 W11 O6 87.7(2) . . ?
O20 W11 O18 154.4(2) . . ?
O20 W11 O19 86.6(2) . . ?
O38 W11 O4 171.3(2) . . ?
O38 W11 O6 101.7(3) . . ?
O38 W11 O18 102.5(3) . . ?
O38 W11 O19 103.4(3) . . ?
O38 W11 O20 103.1(3) . . ?
O7 W12 O4 72.5(2) . . ?
O16 W12 O4 82.9(2) . . ?
O16 W12 O7 88.3(2) . . ?
O17 W12 O4 81.8(2) . . ?
O17 W12 O7 154.1(3) . . ?
O17 W12 O16 84.8(2) . . ?
O18 W12 O4 72.9(2) . . ?
O18 W12 O7 87.3(3) . . ?
O18 W12 O16 155.5(2) . . ?
O18 W12 O17 88.8(2) . . ?
O32 W12 O4 172.4(3) . . ?
O32 W12 O7 103.6(3) . . ?
O32 W12 O16 103.7(3) . . ?
O32 W12 O17 102.4(3) . . ?
O32 W12 O18 100.7(3) . . ?
O41 Cu1 O45 90.9(3) . . ?
O42 Cu1 O41 87.4(3) . . ?
O42 Cu1 O43 95.5(3) . . ?
O42 Cu1 O44 176.7(3) . . ?
O42 Cu1 O45 91.4(3) . . ?
O43 Cu1 O41 176.6(3) . . ?
O43 Cu1 O45 87.4(2) . . ?
O44 Cu1 O41 89.6(3) . . ?
O44 Cu1 O43 87.6(3) . . ?
O44 Cu1 O45 90.0(2) . . ?
O46 Cu2A O31 88.4(4) . . ?
O46 Cu2A O50A 100.2(8) . . ?
O47A Cu2A O31 85.7(7) . . ?
O47A Cu2A O46 89.3(8) . . ?
O47A Cu2A O50A 89.3(11) . . ?
O48A Cu2A O31 83.8(7) . . ?
O48A Cu2A O46 171.6(9) . . ?
O48A Cu2A O47A 86.8(10) . . ?
O48A Cu2A O50A 87.2(10) . . ?
O49A Cu2A O31 91.3(7) . . ?
O49A Cu2A O46 98.9(8) . . ?
O49A Cu2A O47A 171.2(10) . . ?
O49A Cu2A O48A 84.7(10) . . ?
O49A Cu2A O50A 92.3(11) . . ?
O50A Cu2A O31 170.0(8) . . ?
O46 Cu2B O31 86.8(4) . . ?
O46 Cu2B O48B 172.8(9) . . ?
O46 Cu2B O49B 79.1(8) . . ?
O46 Cu2B O50B 91.7(8) . . ?
O47B Cu2B O31 77.6(7) . . ?
O47B Cu2B O46 95.4(8) . . ?
O47B Cu2B O48B 91.8(11) . . ?
O47B Cu2B O49B 163.4(10) . . ?
O47B Cu2B O50B 99.1(11) . . ?
O48B Cu2B O31 94.3(8) . . ?
O48B Cu2B O49B 93.9(10) . . ?
O48B Cu2B O50B 87.7(11) . . ?
O49B Cu2B O31 86.4(7) . . ?
O49B Cu2B O50B 96.7(10) . . ?
O50B Cu2B O31 176.2(8) . . ?
O1 P1 O3 109.7(3) . . ?
O2 P1 O1 109.4(3) . . ?
O2 P1 O3 109.1(3) . . ?
O2 P1 O4 109.3(3) . . ?
O4 P1 O1 109.9(3) . . ?
O4 P1 O3 109.5(3) . . ?
W2 O1 W7 89.20(18) . . ?
W2 O1 W8 88.97(18) . . ?
W7 O1 W8 89.12(19) . . ?
P1 O1 W2 126.3(3) . . ?
P1 O1 W7 125.5(3) . . ?
P1 O1 W8 125.9(3) . . ?
W1 O2 W5 89.20(19) . . ?
W1 O2 W6 89.20(19) . . ?
W6 O2 W5 88.44(18) . . ?
P1 O2 W1 125.9(3) . . ?
P1 O2 W5 126.2(3) . . ?
P1 O2 W6 126.0(3) . . ?
W3 O3 W4 89.01(19) . . ?
W3 O3 W9 89.05(18) . . ?
W9 O3 W4 89.52(18) . . ?
P1 O3 W3 126.1(3) . . ?
P1 O3 W4 126.0(3) . . ?
P1 O3 W9 125.4(3) . . ?
W10 O4 W11 89.00(19) . . ?
W12 O4 W10 88.97(18) . . ?
W12 O4 W11 88.60(19) . . ?
P1 O4 W10 126.2(3) . . ?
P1 O4 W11 125.6(3) . . ?
P1 O4 W12 126.4(3) . . ?
W4 O5 W10 152.1(4) . . ?
W10 O6 W11 126.8(3) . . ?
W10 O7 W12 126.0(3) . . ?
W10 O8 W5 154.4(3) . . ?
W5 O9 W4 152.0(3) . . ?
W6 O10 W5 126.0(3) . . ?
W5 O11 W1 125.9(3) . . ?
W1 O12 W3 152.2(3) . . ?
W1 O13 W2 151.9(3) . . ?
W1 O14 W6 125.9(3) . . ?
W7 O15 W6 152.7(3) . . ?
W6 O16 W12 153.2(3) . . ?
W12 O17 W7 152.4(3) . . ?
W12 O18 W11 126.6(3) . . ?
W11 O19 W8 151.8(3) . . ?
W11 O20 W9 151.5(3) . . ?
W4 O21 W9 126.6(3) . . ?
W9 O22 W3 126.8(3) . . ?
W9 O23 W8 154.2(3) . . ?
W8 O24 W2 125.9(3) . . ?
W8 O25 W7 126.0(3) . . ?
W7 O26 W2 125.8(3) . . ?
W2 O27 W3 153.1(3) . . ?
W4 O28 W3 126.2(3) . . ?
W6 O31 Cu2A 137.6(4) . . ?
W6 O31 Cu2B 119.9(3) . . ?
O50B O48B Cu2B 81.0(14) 3_665 . ?
O50A O49A Cu2A 158(2) 3_665 . ?
O49A O50A Cu2A 88.7(16) 3_665 . ?
Cu2B O50B Cu2B 90.0(9) 3_665 . ?
O48B O50B Cu2B 87.0(13) 3_665 . ?
O48B O50B Cu2B 57.2(11) 3_665 3_665 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O1 W2 O27 W3 57.1(7) . . . . ?
O1 W7 O15 W6 57.0(7) . . . . ?
O1 W7 O26 W2 -1.4(3) . . . . ?
O1 W8 O25 W7 -3.5(3) . . . . ?
O1 P1 O2 W1 58.9(5) . . . . ?
O1 P1 O2 W5 179.4(3) . . . . ?
O1 P1 O2 W6 -61.4(4) . . . . ?
O1 P1 O3 W3 -59.4(5) . . . . ?
O1 P1 O3 W4 -179.7(3) . . . . ?
O1 P1 O3 W9 60.1(4) . . . . ?
O1 P1 O4 W10 -179.8(3) . . . . ?
O1 P1 O4 W11 -60.0(4) . . . . ?
O1 P1 O4 W12 59.3(4) . . . . ?
O2 W1 O13 W2 57.4(7) . . . . ?
O2 W1 O14 W6 -3.1(3) . . . . ?
O2 W5 O9 W4 56.2(7) . . . . ?
O2 W6 O10 W5 -1.9(3) . . . . ?
O2 W6 O16 W12 54.4(7) . . . . ?
O2 P1 O1 W2 -60.8(4) . . . . ?
O2 P1 O1 W7 59.4(4) . . . . ?
O2 P1 O1 W8 179.0(3) . . . . ?
O2 P1 O3 W3 60.4(4) . . . . ?
O2 P1 O3 W4 -59.9(5) . . . . ?
O2 P1 O3 W9 179.9(3) . . . . ?
O2 P1 O4 W10 60.1(5) . . . . ?
O2 P1 O4 W11 179.9(3) . . . . ?
O2 P1 O4 W12 -60.7(5) . . . . ?
O3 W4 O9 W5 -56.4(7) . . . . ?
O3 W9 O22 W3 -2.4(3) . . . . ?
O3 W9 O23 W8 59.3(8) . . . . ?
O3 P1 O1 W2 58.8(4) . . . . ?
O3 P1 O1 W7 179.0(3) . . . . ?
O3 P1 O1 W8 -61.4(4) . . . . ?
O3 P1 O2 W1 -61.1(5) . . . . ?
O3 P1 O2 W5 59.4(5) . . . . ?
O3 P1 O2 W6 178.7(3) . . . . ?
O3 P1 O4 W10 -59.3(4) . . . . ?
O3 P1 O4 W11 60.5(4) . . . . ?
O3 P1 O4 W12 179.9(3) . . . . ?
O4 W10 O8 W5 58.2(8) . . . . ?
O4 W11 O19 W8 -55.5(7) . . . . ?
O4 W11 O20 W9 59.4(7) . . . . ?
O4 W12 O18 W11 -2.0(3) . . . . ?
O4 P1 O1 W2 179.2(3) . . . . ?
O4 P1 O1 W7 -60.6(4) . . . . ?
O4 P1 O1 W8 59.0(4) . . . . ?
O4 P1 O2 W1 179.2(3) . . . . ?
O4 P1 O2 W5 -60.3(5) . . . . ?
O4 P1 O2 W6 59.0(5) . . . . ?
O4 P1 O3 W3 179.9(3) . . . . ?
O4 P1 O3 W4 59.7(5) . . . . ?
O4 P1 O3 W9 -60.6(4) . . . . ?
O5 W4 O9 W5 26.5(7) . . . . ?
O5 W10 O8 W5 -25.5(8) . . . . ?
O6 W10 O8 W5 48.7(12) . . . . ?
O6 W11 O19 W8 -49.6(11) . . . . ?
O6 W11 O20 W9 131.1(7) . . . . ?
O7 W10 O8 W5 130.5(8) . . . . ?
O7 W12 O18 W11 70.6(4) . . . . ?
O8 W5 O9 W4 -26.4(7) . . . . ?
O10 W5 O9 W4 48.1(11) . . . . ?
O10 W6 O16 W12 127.2(8) . . . . ?
O10 W6 O31 Cu2A -32.6(6) . . . . ?
O10 W6 O31 Cu2B -53.9(4) . . . . ?
O11 W1 O13 W2 47.4(11) . . . . ?
O11 W1 O14 W6 69.2(4) . . . . ?
O11 W5 O9 W4 128.6(7) . . . . ?
O12 W1 O13 W2 -26.2(7) . . . . ?
O12 W1 O14 W6 -8.8(9) . . . . ?
O13 W1 O14 W6 -86.5(4) . . . . ?
O13 W2 O27 W3 -26.0(8) . . . . ?
O14 W1 O13 W2 130.1(7) . . . . ?
O14 W6 O10 W5 70.2(4) . . . . ?
O14 W6 O16 W12 42.9(11) . . . . ?
O14 W6 O31 Cu2A 56.6(5) . . . . ?
O14 W6 O31 Cu2B 35.2(4) . . . . ?
O15 W6 O10 W5 -6.0(9) . . . . ?
O15 W6 O16 W12 -28.4(7) . . . . ?
O15 W6 O31 Cu2A 145.9(5) . . . . ?
O15 W6 O31 Cu2B 124.5(3) . . . . ?
O15 W7 O26 W2 -84.4(4) . . . . ?
O16 W6 O10 W5 -85.1(4) . . . . ?
O16 W6 O31 Cu2A -126.3(5) . . . . ?
O16 W6 O31 Cu2B -147.6(3) . . . . ?
O16 W12 O18 W11 -9.3(8) . . . . ?
O17 W7 O15 W6 -25.4(7) . . . . ?
O17 W7 O26 W2 -2.8(8) . . . . ?
O17 W12 O18 W11 -83.8(4) . . . . ?
O18 W11 O19 W8 -127.4(7) . . . . ?
O18 W11 O20 W9 55.2(10) . . . . ?
O19 W8 O25 W7 -87.7(4) . . . . ?
O19 W11 O20 W9 -24.4(7) . . . . ?
O20 W9 O22 W3 -8.4(8) . . . . ?
O20 W9 O23 W8 -24.6(8) . . . . ?
O20 W11 O19 W8 27.4(7) . . . . ?
O21 W4 O9 W5 -49.7(11) . . . . ?
O21 W9 O22 W3 69.9(4) . . . . ?
O21 W9 O23 W8 50.6(11) . . . . ?
O22 W9 O23 W8 131.4(8) . . . . ?
O23 W8 O25 W7 -12.0(8) . . . . ?
O23 W9 O22 W3 -84.7(4) . . . . ?
O24 W2 O27 W3 129.6(8) . . . . ?
O24 W8 O25 W7 68.8(4) . . . . ?
O25 W7 O15 W6 44.9(11) . . . . ?
O25 W7 O26 W2 71.1(4) . . . . ?
O26 W2 O27 W3 48.5(11) . . . . ?
O26 W7 O15 W6 129.4(7) . . . . ?
O28 W4 O9 W5 -128.5(7) . . . . ?
O29 W10 O8 W5 -126.0(8) . . . . ?
O30 W5 O9 W4 -129.3(7) . . . . ?
O31 W6 O10 W5 170.5(4) . . . . ?
O31 W6 O16 W12 -130.4(7) . . . . ?
O32 W12 O18 W11 173.9(4) . . . . ?
O33 W7 O15 W6 -126.7(7) . . . . ?
O33 W7 O26 W2 172.4(4) . . . . ?
O34 W2 O27 W3 -129.2(8) . . . . ?
O35 W1 O13 W2 -128.7(7) . . . . ?
O35 W1 O14 W6 170.1(4) . . . . ?
O37 W4 O9 W5 129.3(7) . . . . ?
O38 W11 O19 W8 130.1(7) . . . . ?
O38 W11 O20 W9 -127.4(7) . . . . ?
O39 W9 O22 W3 171.6(4) . . . . ?
O39 W9 O23 W8 -126.1(8) . . . . ?
O40 W8 O25 W7 169.2(4) . . . . ?

_shelx_SHELXL_version_number     2014/7
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
_exptl_oxdiff_crystal_face_indexfrac_h
_exptl_oxdiff_crystal_face_indexfrac_k
_exptl_oxdiff_crystal_face_indexfrac_l
_exptl_oxdiff_crystal_face_x
_exptl_oxdiff_crystal_face_y
_exptl_oxdiff_crystal_face_z
-16 11 -5 0.2426 -16.1350 11.0429 -4.9553 -0.2615 -0.3431 0.9022
16 -15 -2 0.1298 15.8766 -15.1408 -1.8016 0.4337 0.5667 -0.7005
14 0 -15 0.0862 14.0248 0.1058 -14.7195 0.9465 0.2801 -0.1604
-14 0 14 0.0833 -14.3146 -0.0031 14.3289 -0.9422 -0.2789 0.1855
-4 30 3 0.1639 -3.9856 29.9939 2.9880 0.0671 -0.9825 0.2062
14 -2 13 0.3070 13.9747 -1.9822 13.0139 0.0158 -0.0634 -1.0177
-13 12 -10 0.2470 -12.9737 11.9829 -10.0157 0.0180 -0.2824 0.9233
-1 -31 1 0.1354 -1.0204 -30.9918 1.0098 -0.3733 0.9304 -0.1144
-9 -24 -7 0.2597 -9.0015 -24.0040 -7.0002 -0.3055 0.7956 0.5087
9 -22 10 0.2245 8.9684 -21.9819 10.0162 -0.2492 0.5698 -0.7897
-11 14 -14 0.2427 -10.9664 13.9794 -14.0159 0.2351 -0.2753 0.9666
5 28 -6 0.1609 5.0258 27.9894 -6.0072 0.6396 -0.7458 0.0804
1 31 2 0.1869 1.0156 30.9946 1.9910 0.2749 -0.9746 0.0226
0 -21 -16 0.2663 0.0130 -21.0097 -15.9971 0.3166 0.8791 0.4034
-13 -21 -1 0.2325 -13.0084 -21.0006 -1.0025 -0.6046 0.5962 0.5121
1 -27 -11 0.2064 1.0010 -27.0032 -10.9931 0.1261 0.9941 0.1820

_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_cu_siw_new_19_red_abs
_database_code_depnum_ccdc_archive 'CCDC 1420705'
_audit_update_record             
;
2015-09-02 deposited with the CCDC.
2016-05-19 downloaded from the CCDC.
;
_audit_creation_date             2015-08-24
_audit_creation_method           
;
Olex2 1.2
(compiled 2015.01.26 svn.r3151 for OlexSys, GUI svn.r4998)
;
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Cu2 O50 Si W12, 6(O)'
_chemical_formula_sum            'Cu2 H32 O56 Si W12'
_chemical_formula_weight         3289.62
_chemical_melting_point          ?
_chemical_oxdiff_formula         'Cu2 Si W12 O56 H32'
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/n 1'
_space_group_name_Hall           '-P 2yn'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'

_cell_length_a                   12.9789(6)
_cell_length_b                   22.2778(10)
_cell_length_c                   15.4690(5)
_cell_angle_alpha                90
_cell_angle_beta                 94.527(4)
_cell_angle_gamma                90
_cell_volume                     4458.8(3)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    7851
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      28.8450
_cell_measurement_theta_min      1.8110
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    31.911
_exptl_absorpt_correction_T_max  0.390
_exptl_absorpt_correction_T_min  0.021
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details   
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
Analytical numeric absorption correction using a multifaceted crystal
			model based on expressions derived by R.C. Clark & J.S. Reid.
(Clark, R. C. & Reid, J. S. (1995). Acta Cryst. A51, 887-897)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            'light blue'
_exptl_crystal_colour_modifier   light
_exptl_crystal_colour_primary    blue
_exptl_crystal_density_diffrn    4.900
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       plate
_exptl_crystal_F_000             5760
_exptl_crystal_size_max          0.2839
_exptl_crystal_size_mid          0.1149
_exptl_crystal_size_min          0.0296
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0405
_diffrn_reflns_av_unetI/netI     0.0546
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.900
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       30
_diffrn_reflns_limit_k_min       -29
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            26186
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.900
_diffrn_reflns_theta_full        26.000
_diffrn_reflns_theta_max         29.061
_diffrn_reflns_theta_min         1.606
_diffrn_ambient_temperature      293(2)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 16.1183
_diffrn_detector_type            Eos
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.900
_diffrn_measurement_details      
;
#__ type_ start__ end____ width___ exp.time_
  1 omega  -15.00   15.00   1.0000  104.1100
omega____ theta____ kappa____ phi______ frames
    -      -27.9089  -80.0000 -146.0772 30

#__ type_ start__ end____ width___ exp.time_
  2 omega -102.00    1.00   1.0000  104.1100
omega____ theta____ kappa____ phi______ frames
    -      -27.9089  -57.0000  -90.0000 103

#__ type_ start__ end____ width___ exp.time_
  3 omega -118.00  -35.00   1.0000  104.1100
omega____ theta____ kappa____ phi______ frames
    -      -27.9089  178.0000    0.0000 83

#__ type_ start__ end____ width___ exp.time_
  4 omega  -14.00   46.00   1.0000  104.1100
omega____ theta____ kappa____ phi______ frames
    -      -27.9089   37.0000   30.0000 60

#__ type_ start__ end____ width___ exp.time_
  5 omega -108.00  -18.00   1.0000  104.1100
omega____ theta____ kappa____ phi______ frames
    -      -27.9089  -37.0000   30.0000 90
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Xcalibur, Eos, Gemini ultra'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_UB_11      0.0082907000
_diffrn_orient_matrix_UB_12      0.0309075000
_diffrn_orient_matrix_UB_13      0.0090171000
_diffrn_orient_matrix_UB_21      0.0406595000
_diffrn_orient_matrix_UB_22      -0.0075307000
_diffrn_orient_matrix_UB_23      0.0314732000
_diffrn_orient_matrix_UB_31      0.0358378000
_diffrn_orient_matrix_UB_32      0.0013525000
_diffrn_orient_matrix_UB_33      -0.0322912000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   'Enhance (Mo) X-ray Source'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                8842
_reflns_number_total             10728
_reflns_odcompleteness_completeness 99.98
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     26.32
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_data_collection       
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_data_reduction        
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2008)'
_computing_structure_solution    'ShelXS (Sheldrick, 2008)'
_refine_diff_density_max         3.304
_refine_diff_density_min         -2.804
_refine_diff_density_rms         0.485
_refine_ls_extinction_coef       0.000068(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.081
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     641
_refine_ls_number_reflns         10728
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0505
_refine_ls_R_factor_gt           0.0373
_refine_ls_restrained_S_all      1.081
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0434P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0888
_refine_ls_wR_factor_ref         0.0969
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W -0.05947(3) 0.83483(2) 0.31009(3) 0.01828(11) Uani 1 1 d . . . . .
W2 W 0.10775(3) 0.71539(2) 0.22998(3) 0.01737(10) Uani 1 1 d . . . . .
W3 W -0.05871(3) 0.61032(2) 0.28715(3) 0.01594(10) Uani 1 1 d . . . . .
W4 W -0.22690(3) 0.72945(2) 0.36640(3) 0.01706(10) Uani 1 1 d . . . . .
W5 W -0.13134(3) 0.82826(2) 0.51560(3) 0.01644(10) Uani 1 1 d . . . . .
W6 W 0.14226(3) 0.82044(2) 0.60046(3) 0.01593(10) Uani 1 1 d . . . . .
W7 W 0.21496(3) 0.82350(2) 0.39416(3) 0.01753(10) Uani 1 1 d . . . . .
W8 W 0.29526(3) 0.71327(2) 0.53187(3) 0.01750(11) Uani 1 1 d . . . . .
W9 W -0.04347(3) 0.70394(2) 0.66061(3) 0.01578(10) Uani 1 1 d . . . . .
W10 W -0.13850(3) 0.60386(2) 0.51068(3) 0.01633(10) Uani 1 1 d . . . . .
W11 W 0.10973(3) 0.59639(2) 0.58815(3) 0.01740(10) Uani 1 1 d . . . . .
W12 W 0.19103(3) 0.60503(2) 0.36525(3) 0.01668(10) Uani 1 1 d . . . . .
Cu1 Cu -0.04716(11) 0.99881(8) 0.16201(9) 0.0300(4) Uani 1 1 d . . . . .
Cu2 Cu -0.12928(11) 0.48121(8) 0.10401(9) 0.0290(4) Uani 1 1 d . . . . .
Si1 Si 0.03406(19) 0.71559(13) 0.44736(16) 0.0099(6) Uani 1 1 d . . . . .
O1 O -0.0615(5) 0.7607(3) 0.4202(4) 0.0163(16) Uani 1 1 d . . . . .
O2 O 0.1354(5) 0.7541(4) 0.4808(4) 0.0152(16) Uani 1 1 d . . . . .
O3 O 0.0600(5) 0.6763(3) 0.3627(4) 0.0141(15) Uani 1 1 d . . . . .
O4 O 0.0028(5) 0.6716(3) 0.5238(4) 0.0154(16) Uani 1 1 d . . . . .
O5 O 0.0769(5) 0.8500(3) 0.3627(5) 0.0187(16) Uani 1 1 d . . . . .
O6 O -0.1144(5) 0.8736(4) 0.4087(4) 0.0201(17) Uani 1 1 d . . . . .
O7 O -0.1889(5) 0.7923(4) 0.2926(4) 0.0198(17) Uani 1 1 d . . . . .
O8 O 0.0040(5) 0.7731(4) 0.2461(4) 0.0199(17) Uani 1 1 d . . . . .
O9 O 0.1953(6) 0.7666(4) 0.3039(4) 0.0200(17) Uani 1 1 d . . . . .
O10 O 0.2030(5) 0.6520(4) 0.2618(4) 0.0199(17) Uani 1 1 d . . . . .
O11 O 0.0052(6) 0.6558(4) 0.2005(4) 0.0227(18) Uani 1 1 d . . . . .
O12 O 0.0704(5) 0.5679(4) 0.3076(4) 0.0210(17) Uani 1 1 d . . . . .
O13 O -0.0911(5) 0.5863(3) 0.4013(4) 0.0149(15) Uani 1 1 d . . . . .
O14 O -0.1554(5) 0.6736(4) 0.3000(4) 0.0205(18) Uani 1 1 d . . . . .
O15 O -0.2462(5) 0.7897(3) 0.4543(4) 0.0146(16) Uani 1 1 d . . . . .
O16 O -0.2096(5) 0.6708(4) 0.4571(4) 0.0170(16) Uani 1 1 d . . . . .
O17 O -0.1455(5) 0.6455(4) 0.6218(4) 0.0199(17) Uani 1 1 d . . . . .
O18 O -0.0233(5) 0.5606(4) 0.5668(4) 0.0187(17) Uani 1 1 d . . . . .
O19 O -0.1205(5) 0.7650(4) 0.5960(5) 0.0190(17) Uani 1 1 d . . . . .
O20 O 0.0699(5) 0.7578(4) 0.6530(4) 0.0218(18) Uani 1 1 d . . . . .
O21 O 0.0538(5) 0.6397(3) 0.6829(4) 0.0153(16) Uani 1 1 d . . . . .
O22 O 0.0097(5) 0.8459(3) 0.5493(4) 0.0144(15) Uani 1 1 d . . . . .
O23 O 0.2031(5) 0.8627(4) 0.5078(4) 0.0202(17) Uani 1 1 d . . . . .
O24 O 0.2668(5) 0.7740(3) 0.6137(4) 0.0162(16) Uani 1 1 d . . . . .
O25 O 0.3242(5) 0.7763(4) 0.4510(5) 0.0212(18) Uani 1 1 d . . . . .
O26 O 0.2696(5) 0.6623(4) 0.4315(4) 0.0175(16) Uani 1 1 d . . . . .
O27 O 0.2143(5) 0.6575(4) 0.5880(4) 0.0189(17) Uani 1 1 d . . . . .
O28 O 0.1404(5) 0.5803(4) 0.4740(4) 0.0174(16) Uani 1 1 d . . . . .
O29 O -0.0758(6) 0.8922(4) 0.2375(5) 0.027(2) Uani 1 1 d . . . . .
O30 O 0.1439(6) 0.7322(4) 0.1282(5) 0.0276(19) Uani 1 1 d . . . . .
O31 O -0.1265(6) 0.5587(4) 0.2228(4) 0.0252(19) Uani 1 1 d . . . . .
O32 O -0.3532(6) 0.7185(4) 0.3306(5) 0.026(2) Uani 1 1 d . . . . .
O33 O -0.1939(6) 0.8813(4) 0.5702(5) 0.0258(18) Uani 1 1 d . . . . .
O34 O 0.1627(5) 0.8726(4) 0.6820(4) 0.0206(17) Uani 1 1 d . . . . .
O35 O 0.2872(6) 0.8776(4) 0.3506(5) 0.032(2) Uani 1 1 d . . . . .
O36 O 0.4190(5) 0.6954(4) 0.5668(5) 0.0247(19) Uani 1 1 d . . . . .
O37 O 0.2802(5) 0.5505(4) 0.3511(5) 0.0255(19) Uani 1 1 d . . . . .
O38 O 0.1708(6) 0.5415(4) 0.6487(5) 0.0269(19) Uani 1 1 d . . . . .
O39 O -0.2352(5) 0.5530(4) 0.5180(5) 0.0227(18) Uani 1 1 d . . . . .
O40 O -0.0757(6) 0.7175(4) 0.7640(5) 0.0258(19) Uani 1 1 d . . . . .
O41 O 0.0200(7) 1.0392(5) 0.2644(5) 0.043(3) Uani 1 1 d . . . . .
O42 O 0.0828(6) 0.9598(4) 0.1425(6) 0.038(2) Uani 1 1 d . . . . .
O43 O -0.1200(6) 0.9637(4) 0.0575(5) 0.030(2) Uani 1 1 d . . . . .
O44 O -0.1768(6) 1.0379(4) 0.1904(5) 0.033(2) Uani 1 1 d . . . . .
O45 O -0.0032(7) 1.0825(5) 0.0649(5) 0.037(2) Uani 1 1 d . . . . .
O46 O -0.2780(6) 0.4788(4) 0.1058(6) 0.036(2) Uani 1 1 d . . . . .
O47 O -0.1224(7) 0.4000(4) 0.1556(5) 0.035(2) Uani 1 1 d . . . . .
O48 O 0.0202(6) 0.4846(4) 0.1088(5) 0.031(2) Uani 1 1 d . . . . .
O49 O -0.1369(7) 0.5549(4) 0.0311(5) 0.035(2) Uani 1 1 d . . . . .
O50 O -0.1099(6) 0.4244(5) -0.0393(6) 0.042(3) Uani 1 1 d . . . . .
O51W O 0.0900(8) 0.9720(5) 0.4832(7) 0.056(3) Uani 1 1 d . . . . .
O52W O 0.1231(7) 0.4562(4) 0.2578(5) 0.033(2) Uani 1 1 d . . . . .
O53W O 0.1108(7) 0.8540(5) 0.0783(7) 0.051(3) Uani 1 1 d . . . . .
O54W O 0.4510(8) 0.6552(5) 0.2918(7) 0.053(3) Uani 1 1 d . . . . .
O55W O 0.2048(8) 1.0036(6) 0.3399(7) 0.059(3) Uani 1 1 d . . . . .
O56W O 0.0323(7) 0.6772(5) -0.0434(6) 0.046(3) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O1 2.374(7) . ?
W1 O5 1.919(7) . ?
W1 O6 1.938(7) . ?
W1 O7 1.928(7) . ?
W1 O8 1.917(8) . ?
W1 O29 1.703(8) . ?
W2 O3 2.357(7) . ?
W2 O8 1.893(8) . ?
W2 O9 1.923(7) . ?
W2 O10 1.915(8) . ?
W2 O11 1.909(8) . ?
W2 O30 1.719(7) . ?
W3 O3 2.369(7) . ?
W3 O11 1.920(8) . ?
W3 O12 1.928(7) . ?
W3 O13 1.923(7) . ?
W3 O14 1.908(8) . ?
W3 O31 1.718(7) . ?
W4 O1 2.346(7) . ?
W4 O7 1.897(8) . ?
W4 O14 1.901(8) . ?
W4 O15 1.940(7) . ?
W4 O16 1.917(7) . ?
W4 O32 1.706(7) . ?
W5 O1 2.339(8) . ?
W5 O6 1.964(7) . ?
W5 O15 1.908(7) . ?
W5 O19 1.877(8) . ?
W5 O22 1.904(7) . ?
W5 O33 1.696(8) . ?
W6 O2 2.364(7) . ?
W6 O20 1.900(8) . ?
W6 O22 1.922(7) . ?
W6 O23 1.935(7) . ?
W6 O24 1.916(7) . ?
W6 O34 1.720(8) . ?
W7 O2 2.339(7) . ?
W7 O5 1.912(7) . ?
W7 O9 1.888(7) . ?
W7 O23 1.980(7) . ?
W7 O25 1.922(7) . ?
W7 O35 1.698(9) . ?
W8 O2 2.345(6) . ?
W8 O24 1.909(7) . ?
W8 O25 1.937(8) . ?
W8 O26 1.932(7) . ?
W8 O27 1.883(8) . ?
W8 O36 1.701(7) . ?
W9 O4 2.358(7) . ?
W9 O17 1.919(7) . ?
W9 O19 1.921(7) . ?
W9 O20 1.909(8) . ?
W9 O21 1.921(7) . ?
W9 O40 1.712(8) . ?
W10 O4 2.371(7) . ?
W10 O13 1.887(7) . ?
W10 O16 1.908(7) . ?
W10 O17 1.961(7) . ?
W10 O18 1.927(7) . ?
W10 O39 1.701(8) . ?
W11 O4 2.347(7) . ?
W11 O18 1.907(7) . ?
W11 O21 1.943(7) . ?
W11 O27 1.923(7) . ?
W11 O28 1.875(7) . ?
W11 O38 1.697(8) . ?
W12 O3 2.325(7) . ?
W12 O10 1.929(8) . ?
W12 O12 1.925(7) . ?
W12 O26 1.884(7) . ?
W12 O28 1.934(7) . ?
W12 O37 1.704(8) . ?
Cu1 O29 2.686(9) . ?
Cu1 O41 1.964(8) . ?
Cu1 O42 1.942(9) . ?
Cu1 O43 1.970(8) . ?
Cu1 O44 1.975(8) . ?
Cu1 O45 2.489(10) . ?
Cu2 O31 2.519(8) . ?
Cu2 O46 1.933(8) . ?
Cu2 O47 1.976(9) . ?
Cu2 O48 1.937(8) . ?
Cu2 O49 1.989(9) . ?
Cu2 O50 2.581(9) . ?
Si1 O1 1.626(7) . ?
Si1 O2 1.621(7) . ?
Si1 O3 1.633(7) . ?
Si1 O4 1.612(8) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O5 W1 O1 83.1(3) . . ?
O5 W1 O6 88.4(3) . . ?
O5 W1 O7 155.5(3) . . ?
O6 W1 O1 73.7(3) . . ?
O7 W1 O1 72.6(3) . . ?
O7 W1 O6 87.6(3) . . ?
O8 W1 O1 84.3(3) . . ?
O8 W1 O5 85.7(3) . . ?
O8 W1 O6 157.8(3) . . ?
O8 W1 O7 88.9(3) . . ?
O29 W1 O1 170.7(3) . . ?
O29 W1 O5 102.2(4) . . ?
O29 W1 O6 98.6(4) . . ?
O29 W1 O7 102.4(3) . . ?
O29 W1 O8 103.5(4) . . ?
O8 W2 O3 84.1(3) . . ?
O8 W2 O9 84.9(3) . . ?
O8 W2 O10 156.7(3) . . ?
O8 W2 O11 90.8(3) . . ?
O9 W2 O3 83.4(3) . . ?
O10 W2 O3 73.3(3) . . ?
O10 W2 O9 86.9(3) . . ?
O11 W2 O3 74.0(3) . . ?
O11 W2 O9 157.3(3) . . ?
O11 W2 O10 88.4(3) . . ?
O30 W2 O3 170.9(4) . . ?
O30 W2 O8 102.8(4) . . ?
O30 W2 O9 103.0(4) . . ?
O30 W2 O10 100.3(4) . . ?
O30 W2 O11 99.7(4) . . ?
O11 W3 O3 73.6(3) . . ?
O11 W3 O12 87.4(3) . . ?
O11 W3 O13 157.8(3) . . ?
O12 W3 O3 72.5(3) . . ?
O13 W3 O3 84.3(3) . . ?
O13 W3 O12 87.9(3) . . ?
O14 W3 O3 84.1(3) . . ?
O14 W3 O11 90.4(3) . . ?
O14 W3 O12 156.2(3) . . ?
O14 W3 O13 85.2(3) . . ?
O31 W3 O3 169.9(3) . . ?
O31 W3 O11 100.3(3) . . ?
O31 W3 O12 99.6(4) . . ?
O31 W3 O13 101.9(3) . . ?
O31 W3 O14 104.1(3) . . ?
O7 W4 O1 73.7(3) . . ?
O7 W4 O14 89.8(3) . . ?
O7 W4 O15 88.0(3) . . ?
O7 W4 O16 157.3(3) . . ?
O14 W4 O1 85.1(3) . . ?
O14 W4 O15 157.9(3) . . ?
O14 W4 O16 85.1(3) . . ?
O15 W4 O1 73.2(3) . . ?
O16 W4 O1 83.8(3) . . ?
O16 W4 O15 88.4(3) . . ?
O32 W4 O1 170.6(4) . . ?
O32 W4 O7 101.5(3) . . ?
O32 W4 O14 103.2(4) . . ?
O32 W4 O15 98.7(3) . . ?
O32 W4 O16 101.2(3) . . ?
O6 W5 O1 74.0(3) . . ?
O15 W5 O1 73.9(3) . . ?
O15 W5 O6 87.1(3) . . ?
O19 W5 O1 85.6(3) . . ?
O19 W5 O6 159.4(3) . . ?
O19 W5 O15 90.3(3) . . ?
O19 W5 O22 87.4(3) . . ?
O22 W5 O1 83.9(3) . . ?
O22 W5 O6 87.4(3) . . ?
O22 W5 O15 157.8(3) . . ?
O33 W5 O1 170.6(3) . . ?
O33 W5 O6 98.7(4) . . ?
O33 W5 O15 100.1(3) . . ?
O33 W5 O19 101.9(4) . . ?
O33 W5 O22 101.9(3) . . ?
O20 W6 O2 83.5(3) . . ?
O20 W6 O22 86.4(3) . . ?
O20 W6 O23 156.8(3) . . ?
O20 W6 O24 90.0(3) . . ?
O22 W6 O2 83.4(3) . . ?
O22 W6 O23 87.4(3) . . ?
O23 W6 O2 73.5(3) . . ?
O24 W6 O2 74.1(2) . . ?
O24 W6 O22 157.4(3) . . ?
O24 W6 O23 87.2(3) . . ?
O34 W6 O2 172.0(3) . . ?
O34 W6 O20 103.6(3) . . ?
O34 W6 O22 100.6(3) . . ?
O34 W6 O23 99.6(3) . . ?
O34 W6 O24 101.9(3) . . ?
O5 W7 O2 84.4(3) . . ?
O5 W7 O23 87.3(3) . . ?
O5 W7 O25 158.1(3) . . ?
O9 W7 O2 86.6(3) . . ?
O9 W7 O5 87.1(3) . . ?
O9 W7 O23 159.6(3) . . ?
O9 W7 O25 91.3(3) . . ?
O23 W7 O2 73.4(3) . . ?
O25 W7 O2 73.7(3) . . ?
O25 W7 O23 86.7(3) . . ?
O35 W7 O2 168.1(3) . . ?
O35 W7 O5 102.5(4) . . ?
O35 W7 O9 103.3(4) . . ?
O35 W7 O23 97.1(4) . . ?
O35 W7 O25 99.2(4) . . ?
O24 W8 O2 74.7(3) . . ?
O24 W8 O25 88.4(3) . . ?
O24 W8 O26 156.9(3) . . ?
O25 W8 O2 73.3(3) . . ?
O26 W8 O2 82.3(3) . . ?
O26 W8 O25 86.4(3) . . ?
O27 W8 O2 84.3(3) . . ?
O27 W8 O24 91.0(3) . . ?
O27 W8 O25 156.9(3) . . ?
O27 W8 O26 85.2(3) . . ?
O36 W8 O2 170.4(4) . . ?
O36 W8 O24 100.5(3) . . ?
O36 W8 O25 98.5(4) . . ?
O36 W8 O26 102.5(3) . . ?
O36 W8 O27 104.3(4) . . ?
O17 W9 O4 74.3(3) . . ?
O17 W9 O19 90.0(3) . . ?
O17 W9 O21 88.8(3) . . ?
O19 W9 O4 84.7(3) . . ?
O19 W9 O21 158.2(3) . . ?
O20 W9 O4 83.4(3) . . ?
O20 W9 O17 157.4(3) . . ?
O20 W9 O19 84.0(3) . . ?
O20 W9 O21 88.9(3) . . ?
O21 W9 O4 73.9(3) . . ?
O40 W9 O4 172.3(3) . . ?
O40 W9 O17 101.5(4) . . ?
O40 W9 O19 101.8(4) . . ?
O40 W9 O20 101.1(4) . . ?
O40 W9 O21 99.8(3) . . ?
O13 W10 O4 84.5(3) . . ?
O13 W10 O16 87.3(3) . . ?
O13 W10 O17 157.6(3) . . ?
O13 W10 O18 90.2(3) . . ?
O16 W10 O4 83.3(3) . . ?
O16 W10 O17 87.5(3) . . ?
O16 W10 O18 156.6(3) . . ?
O17 W10 O4 73.3(3) . . ?
O18 W10 O4 73.3(3) . . ?
O18 W10 O17 86.0(3) . . ?
O39 W10 O4 171.1(3) . . ?
O39 W10 O13 102.5(3) . . ?
O39 W10 O16 102.4(3) . . ?
O39 W10 O17 99.9(3) . . ?
O39 W10 O18 100.8(4) . . ?
O18 W11 O4 74.2(3) . . ?
O18 W11 O21 87.2(3) . . ?
O18 W11 O27 157.7(3) . . ?
O21 W11 O4 73.8(3) . . ?
O27 W11 O4 83.5(3) . . ?
O27 W11 O21 87.4(3) . . ?
O28 W11 O4 84.2(3) . . ?
O28 W11 O18 90.8(3) . . ?
O28 W11 O21 157.7(3) . . ?
O28 W11 O27 86.1(3) . . ?
O38 W11 O4 169.4(3) . . ?
O38 W11 O18 99.9(4) . . ?
O38 W11 O21 97.3(3) . . ?
O38 W11 O27 102.2(3) . . ?
O38 W11 O28 104.9(4) . . ?
O10 W12 O3 73.8(3) . . ?
O10 W12 O28 158.7(3) . . ?
O12 W12 O3 73.6(3) . . ?
O12 W12 O10 88.0(3) . . ?
O12 W12 O28 87.7(3) . . ?
O26 W12 O3 84.9(3) . . ?
O26 W12 O10 90.5(3) . . ?
O26 W12 O12 158.0(3) . . ?
O26 W12 O28 85.8(3) . . ?
O28 W12 O3 84.9(3) . . ?
O37 W12 O3 171.2(3) . . ?
O37 W12 O10 100.4(3) . . ?
O37 W12 O12 99.8(4) . . ?
O37 W12 O26 102.0(3) . . ?
O37 W12 O28 100.9(4) . . ?
O41 Cu1 O29 97.0(4) . . ?
O41 Cu1 O43 175.9(4) . . ?
O41 Cu1 O44 87.2(4) . . ?
O41 Cu1 O45 92.0(4) . . ?
O42 Cu1 O29 79.8(3) . . ?
O42 Cu1 O41 89.7(4) . . ?
O42 Cu1 O43 93.5(4) . . ?
O42 Cu1 O44 176.1(4) . . ?
O42 Cu1 O45 89.9(4) . . ?
O43 Cu1 O29 86.1(3) . . ?
O43 Cu1 O44 89.7(3) . . ?
O43 Cu1 O45 85.4(3) . . ?
O44 Cu1 O29 98.3(3) . . ?
O44 Cu1 O45 92.5(4) . . ?
O45 Cu1 O29 166.2(3) . . ?
O31 Cu2 O50 164.9(3) . . ?
O46 Cu2 O31 88.0(3) . . ?
O46 Cu2 O47 89.0(4) . . ?
O46 Cu2 O48 176.9(4) . . ?
O46 Cu2 O49 91.5(4) . . ?
O46 Cu2 O50 99.4(3) . . ?
O47 Cu2 O31 109.6(3) . . ?
O47 Cu2 O49 169.3(4) . . ?
O47 Cu2 O50 83.9(4) . . ?
O48 Cu2 O31 89.4(3) . . ?
O48 Cu2 O47 90.4(4) . . ?
O48 Cu2 O49 89.7(4) . . ?
O48 Cu2 O50 83.5(3) . . ?
O49 Cu2 O31 81.1(3) . . ?
O49 Cu2 O50 85.5(4) . . ?
O1 Si1 O3 109.0(4) . . ?
O2 Si1 O1 109.7(4) . . ?
O2 Si1 O3 109.1(4) . . ?
O4 Si1 O1 109.5(4) . . ?
O4 Si1 O2 109.5(4) . . ?
O4 Si1 O3 110.0(4) . . ?
W4 O1 W1 90.8(2) . . ?
W5 O1 W1 91.9(3) . . ?
W5 O1 W4 91.5(3) . . ?
Si1 O1 W1 124.3(4) . . ?
Si1 O1 W4 124.4(4) . . ?
Si1 O1 W5 124.1(3) . . ?
W7 O2 W6 92.6(3) . . ?
W7 O2 W8 91.7(2) . . ?
W8 O2 W6 90.1(2) . . ?
Si1 O2 W6 124.1(4) . . ?
Si1 O2 W7 123.4(3) . . ?
Si1 O2 W8 125.2(4) . . ?
W2 O3 W3 90.3(2) . . ?
W12 O3 W2 91.4(2) . . ?
W12 O3 W3 91.8(3) . . ?
Si1 O3 W2 125.8(4) . . ?
Si1 O3 W3 124.1(4) . . ?
Si1 O3 W12 123.3(3) . . ?
W9 O4 W10 91.2(2) . . ?
W11 O4 W9 91.2(2) . . ?
W11 O4 W10 90.5(3) . . ?
Si1 O4 W9 124.7(4) . . ?
Si1 O4 W10 124.2(3) . . ?
Si1 O4 W11 124.8(4) . . ?
W7 O5 W1 150.2(4) . . ?
W1 O6 W5 120.4(4) . . ?
W4 O7 W1 122.9(3) . . ?
W2 O8 W1 153.4(4) . . ?
W7 O9 W2 151.4(4) . . ?
W2 O10 W12 121.4(4) . . ?
W2 O11 W3 122.1(4) . . ?
W12 O12 W3 122.0(4) . . ?
W10 O13 W3 151.2(4) . . ?
W4 O14 W3 153.3(4) . . ?
W5 O15 W4 121.4(4) . . ?
W10 O16 W4 151.1(4) . . ?
W9 O17 W10 121.1(4) . . ?
W11 O18 W10 121.9(4) . . ?
W5 O19 W9 152.2(4) . . ?
W6 O20 W9 153.8(4) . . ?
W9 O21 W11 120.9(3) . . ?
W5 O22 W6 149.5(4) . . ?
W6 O23 W7 120.5(4) . . ?
W8 O24 W6 121.2(3) . . ?
W7 O25 W8 121.2(4) . . ?
W12 O26 W8 152.5(4) . . ?
W8 O27 W11 152.5(4) . . ?
W11 O28 W12 151.2(5) . . ?
W1 O29 Cu1 159.4(4) . . ?
W3 O31 Cu2 149.2(4) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O1 W4 O7 W1 -1.1(4) . . . . ?
O1 W5 O19 W9 54.4(9) . . . . ?
O1 Si1 O2 W6 59.7(5) . . . . ?
O1 Si1 O2 W7 -61.0(5) . . . . ?
O1 Si1 O2 W8 178.3(4) . . . . ?
O1 Si1 O3 W2 58.9(5) . . . . ?
O1 Si1 O3 W3 -61.0(5) . . . . ?
O1 Si1 O3 W12 179.6(4) . . . . ?
O1 Si1 O4 W9 -59.8(5) . . . . ?
O1 Si1 O4 W10 60.4(6) . . . . ?
O1 Si1 O4 W11 179.5(4) . . . . ?
O2 W7 O9 W2 56.3(9) . . . . ?
O2 W8 O27 W11 58.3(9) . . . . ?
O2 Si1 O1 W1 60.4(5) . . . . ?
O2 Si1 O1 W4 179.6(4) . . . . ?
O2 Si1 O1 W5 -60.3(5) . . . . ?
O2 Si1 O3 W2 -61.0(5) . . . . ?
O2 Si1 O3 W3 179.2(4) . . . . ?
O2 Si1 O3 W12 59.8(5) . . . . ?
O2 Si1 O4 W9 60.6(5) . . . . ?
O2 Si1 O4 W10 -179.3(4) . . . . ?
O2 Si1 O4 W11 -60.2(5) . . . . ?
O3 W2 O8 W1 56.5(10) . . . . ?
O3 W3 O31 Cu2 -1(3) . . . . ?
O3 W12 O26 W8 60.1(9) . . . . ?
O3 Si1 O1 W1 -59.1(5) . . . . ?
O3 Si1 O1 W4 60.2(5) . . . . ?
O3 Si1 O1 W5 -179.7(4) . . . . ?
O3 Si1 O2 W6 179.1(4) . . . . ?
O3 Si1 O2 W7 58.3(5) . . . . ?
O3 Si1 O2 W8 -62.3(5) . . . . ?
O3 Si1 O4 W9 -179.5(4) . . . . ?
O3 Si1 O4 W10 -59.4(5) . . . . ?
O3 Si1 O4 W11 59.7(5) . . . . ?
O4 W10 O13 W3 -60.2(8) . . . . ?
O4 W11 O28 W12 58.0(8) . . . . ?
O4 Si1 O1 W1 -179.5(4) . . . . ?
O4 Si1 O1 W4 -60.2(5) . . . . ?
O4 Si1 O1 W5 59.9(5) . . . . ?
O4 Si1 O2 W6 -60.5(6) . . . . ?
O4 Si1 O2 W7 178.7(4) . . . . ?
O4 Si1 O2 W8 58.1(5) . . . . ?
O4 Si1 O3 W2 179.0(4) . . . . ?
O4 Si1 O3 W3 59.1(5) . . . . ?
O4 Si1 O3 W12 -60.3(5) . . . . ?
O5 W1 O29 Cu1 -20.4(13) . . . . ?
O5 W7 O9 W2 -28.3(9) . . . . ?
O6 W1 O29 Cu1 69.8(12) . . . . ?
O6 W5 O19 W9 45.8(15) . . . . ?
O7 W1 O29 Cu1 159.3(12) . . . . ?
O8 W1 O29 Cu1 -108.9(12) . . . . ?
O9 W2 O8 W1 -27.3(10) . . . . ?
O10 W2 O8 W1 42.5(16) . . . . ?
O10 W12 O26 W8 133.9(9) . . . . ?
O11 W2 O8 W1 130.4(10) . . . . ?
O11 W3 O31 Cu2 50.7(9) . . . . ?
O12 W3 O31 Cu2 -38.4(9) . . . . ?
O12 W12 O26 W8 48.1(15) . . . . ?
O13 W3 O31 Cu2 -128.3(8) . . . . ?
O14 W3 O31 Cu2 143.7(8) . . . . ?
O14 W4 O7 W1 -86.0(5) . . . . ?
O15 W4 O7 W1 72.0(5) . . . . ?
O15 W5 O19 W9 128.3(9) . . . . ?
O16 W4 O7 W1 -9.2(12) . . . . ?
O16 W10 O13 W3 23.4(8) . . . . ?
O17 W10 O13 W3 -53.4(12) . . . . ?
O18 W10 O13 W3 -133.4(8) . . . . ?
O18 W11 O28 W12 132.0(8) . . . . ?
O21 W11 O28 W12 47.5(13) . . . . ?
O22 W5 O19 W9 -29.7(9) . . . . ?
O23 W7 O9 W2 46.0(15) . . . . ?
O24 W8 O27 W11 132.7(10) . . . . ?
O25 W7 O9 W2 129.9(9) . . . . ?
O25 W8 O27 W11 44.5(15) . . . . ?
O26 W8 O27 W11 -24.5(9) . . . . ?
O27 W11 O28 W12 -25.9(8) . . . . ?
O28 W12 O26 W8 -25.1(9) . . . . ?
O30 W2 O8 W1 -129.5(10) . . . . ?
O32 W4 O7 W1 170.5(5) . . . . ?
O33 W5 O19 W9 -131.3(9) . . . . ?
O35 W7 O9 W2 -130.4(9) . . . . ?
O36 W8 O27 W11 -126.2(9) . . . . ?
O37 W12 O26 W8 -125.4(9) . . . . ?
O38 W11 O28 W12 -127.5(8) . . . . ?
O39 W10 O13 W3 125.5(8) . . . . ?

_shelx_SHELXL_version_number     2014/7
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
_exptl_oxdiff_crystal_face_indexfrac_h
_exptl_oxdiff_crystal_face_indexfrac_k
_exptl_oxdiff_crystal_face_indexfrac_l
_exptl_oxdiff_crystal_face_x
_exptl_oxdiff_crystal_face_y
_exptl_oxdiff_crystal_face_z
14 1 -15 0.0575 13.9796 1.1109 -15.0445 0.0146 0.0865 0.9883
-14 -1 15 0.0575 -13.9796 -1.1109 15.0445 -0.0146 -0.0865 -0.9883
-2 1 -21 0.1079 -2.0039 1.0399 -21.0073 -0.1739 -0.7505 0.6079
2 -1 21 0.1079 2.0039 -1.0399 21.0073 0.1739 0.7505 -0.6079
16 0 8 0.1374 15.9840 0.0659 7.9641 0.2064 0.9001 0.3157
-16 0 -8 0.1374 -15.9840 -0.0659 -7.9641 -0.2064 -0.9001 -0.3157
0 32 0 0.0203 -0.0423 31.8973 0.0022 0.9855 -0.2419 0.0416
0 -32 0 0.0093 0.0423 -31.8973 -0.0022 -0.9855 0.2419 -0.0416

_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_sb974_cu_siw_13_red_abs
_database_code_depnum_ccdc_archive 'CCDC 1420706'
_audit_update_record             
;
2015-08-26 deposited with the CCDC.
2016-05-19 downloaded from the CCDC.
;
_audit_creation_date             2015-06-16
_audit_creation_method           
;
Olex2 1.2
(compiled 2015.01.26 svn.r3151 for OlexSys, GUI svn.r4998)
;
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Cu2 O50 Si W12, 6(O)'
_chemical_formula_sum            'Cu2 H32 O56 Si W12'
_chemical_formula_weight         3289.62
_chemical_melting_point          ?
_chemical_oxdiff_formula         'Cu2 Si W12 O56'
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   12.8897(4)
_cell_length_b                   14.0070(5)
_cell_length_c                   15.3382(4)
_cell_angle_alpha                63.169(3)
_cell_angle_beta                 71.079(3)
_cell_angle_gamma                63.827(3)
_cell_volume                     2190.49(15)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    15926
_cell_measurement_temperature    125(2)
_cell_measurement_theta_max      28.7490
_cell_measurement_theta_min      1.8290
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    32.478
_exptl_absorpt_correction_T_max  0.099
_exptl_absorpt_correction_T_min  0.020
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details   
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
Analytical numeric absorption correction using a multifaceted crystal
			model based on expressions derived by R.C. Clark & J.S. Reid.
(Clark, R. C. & Reid, J. S. (1995). Acta Cryst. A51, 887-897)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            'light blue'
_exptl_crystal_colour_modifier   light
_exptl_crystal_colour_primary    blue
_exptl_crystal_density_diffrn    4.988
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       prism
_exptl_crystal_F_000             2880
_exptl_crystal_size_max          0.4353
_exptl_crystal_size_mid          0.2037
_exptl_crystal_size_min          0.1372
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0349
_diffrn_reflns_av_unetI/netI     0.0335
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.915
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            37397
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.915
_diffrn_reflns_theta_full        26.000
_diffrn_reflns_theta_max         28.882
_diffrn_reflns_theta_min         1.782
_diffrn_ambient_environment      N~2~
_diffrn_ambient_temperature      125(2)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 16.1183
_diffrn_detector_type            Eos
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.915
_diffrn_measurement_details      
;
#__ type_ start__ end____ width___ exp.time_
  1 omega   84.00  118.00   1.0000   11.4750
omega____ theta____ kappa____ phi______ frames
    -       27.2058  178.0000   60.0000 34

#__ type_ start__ end____ width___ exp.time_
  2 omega   70.00  116.00   1.0000   11.4750
omega____ theta____ kappa____ phi______ frames
    -       27.2058  178.0000  -90.0000 46

#__ type_ start__ end____ width___ exp.time_
  3 omega -115.00  -73.00   1.0000   11.4750
omega____ theta____ kappa____ phi______ frames
    -      -27.9871  178.0000  -60.0000 42

#__ type_ start__ end____ width___ exp.time_
  4 omega  -35.00   52.00   1.0000   11.4750
omega____ theta____ kappa____ phi______ frames
    -      -27.9871   37.0000  150.0000 87

#__ type_ start__ end____ width___ exp.time_
  5 omega  -49.00   51.00   1.0000   11.4750
omega____ theta____ kappa____ phi______ frames
    -      -27.9871   37.0000   60.0000 100

#__ type_ start__ end____ width___ exp.time_
  6 omega  -99.00   -7.00   1.0000   11.4750
omega____ theta____ kappa____ phi______ frames
    -      -27.9871  -57.0000 -180.0000 92

#__ type_ start__ end____ width___ exp.time_
  7 omega  -86.00   -1.00   1.0000   11.4750
omega____ theta____ kappa____ phi______ frames
    -      -27.9871  -37.0000 -120.0000 85

#__ type_ start__ end____ width___ exp.time_
  8 omega  -41.00    2.00   1.0000   11.4750
omega____ theta____ kappa____ phi______ frames
    -       27.2058  126.0000 -128.3268 43

#__ type_ start__ end____ width___ exp.time_
  9 omega -102.00  -14.00   1.0000   11.4750
omega____ theta____ kappa____ phi______ frames
    -      -27.9871  -57.0000  150.0000 88

#__ type_ start__ end____ width___ exp.time_
 10 omega  -49.00   52.00   1.0000   11.4750
omega____ theta____ kappa____ phi______ frames
    -      -27.9871   37.0000 -180.0000 101

#__ type_ start__ end____ width___ exp.time_
 11 omega -108.00   13.00   1.0000   11.4750
omega____ theta____ kappa____ phi______ frames
    -      -27.9871  -77.0000  -60.0000 121

#__ type_ start__ end____ width___ exp.time_
 12 omega  -49.00   52.00   1.0000   11.4750
omega____ theta____ kappa____ phi______ frames
    -      -27.9871   37.0000  -30.0000 101

#__ type_ start__ end____ width___ exp.time_
 13 omega -108.00   13.00   1.0000   11.4750
omega____ theta____ kappa____ phi______ frames
    -      -27.9871  -77.0000   60.0000 121
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Xcalibur, Eos, Gemini ultra'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_UB_11      0.0479045000
_diffrn_orient_matrix_UB_12      -0.0459220000
_diffrn_orient_matrix_UB_13      -0.0109495000
_diffrn_orient_matrix_UB_21      -0.0027446000
_diffrn_orient_matrix_UB_22      0.0308188000
_diffrn_orient_matrix_UB_23      -0.0512141000
_diffrn_orient_matrix_UB_31      0.0393873000
_diffrn_orient_matrix_UB_32      0.0246741000
_diffrn_orient_matrix_UB_33      -0.0031779000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   'Enhance (Mo) X-ray Source'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                9653
_reflns_number_total             10548
_reflns_odcompleteness_completeness 100.00
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     26.32
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_data_collection       
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_data_reduction        
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2008)'
_computing_structure_solution    'ShelXS (Sheldrick, 2008)'
_refine_diff_density_max         1.684
_refine_diff_density_min         -1.537
_refine_diff_density_rms         0.288
_refine_ls_extinction_coef       0.000185(9)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.154
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     641
_refine_ls_number_reflns         10548
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0310
_refine_ls_R_factor_gt           0.0266
_refine_ls_restrained_S_all      1.154
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0183P)²+9.5779P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0576
_refine_ls_wR_factor_ref         0.0590
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.47090(3) 0.41458(2) 0.28571(2) 0.00969(6) Uani 1 1 d . . . . .
W2 W 0.22074(3) 0.47854(2) 0.43850(2) 0.00969(6) Uani 1 1 d . . . . .
W3 W 0.30360(3) 0.68905(2) 0.45835(2) 0.01018(6) Uani 1 1 d . . . . .
W4 W 0.55388(3) 0.62439(2) 0.30547(2) 0.01019(7) Uani 1 1 d . . . . .
W5 W 0.54819(3) 0.63955(2) 0.06014(2) 0.00955(6) Uani 1 1 d . . . . .
W6 W 0.21193(3) 0.50021(2) 0.21477(2) 0.00939(6) Uani 1 1 d . . . . .
W7 W 0.29248(3) 0.72174(2) -0.01037(2) 0.01002(6) Uani 1 1 d . . . . .
W8 W 0.36539(3) 0.91451(2) 0.00620(2) 0.00953(6) Uani 1 1 d . . . . .
W9 W 0.01398(3) 0.80189(2) 0.15480(2) 0.01012(6) Uani 1 1 d . . . . .
W10 W 0.02187(3) 0.77900(2) 0.37998(2) 0.01012(6) Uani 1 1 d . . . . .
W11 W 0.37253(3) 0.89673(2) 0.25108(2) 0.01043(7) Uani 1 1 d . . . . .
W12 W 0.08836(3) 0.99039(2) 0.17564(2) 0.01022(6) Uani 1 1 d . . . . .
Cu1 Cu 0.64647(8) 0.07946(8) 0.37995(7) 0.0155(2) Uani 1 1 d . . . . .
Cu2 Cu -0.04195(8) 1.33200(8) 0.15613(7) 0.0154(2) Uani 1 1 d . . . . .
Si1 Si 0.28824(16) 0.70452(15) 0.22671(14) 0.0059(4) Uani 1 1 d . . . . .
O1 O 0.2952(4) 0.5719(4) 0.2743(4) 0.0083(10) Uani 1 1 d . . . . .
O2 O 0.3558(4) 0.7229(4) 0.2886(4) 0.0112(10) Uani 1 1 d . . . . .
O3 O 0.3507(4) 0.7339(4) 0.1119(3) 0.0071(10) Uani 1 1 d . . . . .
O4 O 0.1524(4) 0.7874(4) 0.2334(4) 0.0091(10) Uani 1 1 d . . . . .
O5 O 0.5195(4) 0.5045(4) 0.1535(4) 0.0120(10) Uani 1 1 d . . . . .
O6 O 0.3694(4) 0.3930(4) 0.2348(4) 0.0111(10) Uani 1 1 d . . . . .
O7 O 0.5215(4) 0.4949(4) 0.3250(4) 0.0116(11) Uani 1 1 d . . . . .
O8 O 0.3744(4) 0.3770(4) 0.4125(4) 0.0113(10) Uani 1 1 d . . . . .
O9 O 0.1688(4) 0.4436(4) 0.3568(4) 0.0112(10) Uani 1 1 d . . . . .
O10 O 0.0899(4) 0.6197(4) 0.4157(4) 0.0112(10) Uani 1 1 d . . . . .
O11 O 0.2852(4) 0.5584(4) 0.4688(4) 0.0123(11) Uani 1 1 d . . . . .
O12 O 0.4694(4) 0.6198(4) 0.4347(4) 0.0140(11) Uani 1 1 d . . . . .
O13 O 0.3268(4) 0.8349(4) 0.3939(4) 0.0121(11) Uani 1 1 d . . . . .
O14 O 0.1481(4) 0.7697(4) 0.4260(4) 0.0115(10) Uani 1 1 d . . . . .
O15 O -0.0576(4) 0.7886(4) 0.2891(4) 0.0100(10) Uani 1 1 d . . . . .
O16 O -0.0002(4) 0.9407(4) 0.3047(4) 0.0112(10) Uani 1 1 d . . . . .
O17 O -0.0052(4) 0.9543(4) 0.1277(4) 0.0120(11) Uani 1 1 d . . . . .
O18 O 0.2075(4) 0.9731(4) 0.0659(4) 0.0124(11) Uani 1 1 d . . . . .
O19 O 0.2108(4) 0.9609(4) 0.2389(4) 0.0125(11) Uani 1 1 d . . . . .
O20 O 0.4058(4) 0.9086(4) 0.1182(4) 0.0109(10) Uani 1 1 d . . . . .
O21 O 0.5174(4) 0.8022(4) -0.0108(4) 0.0105(10) Uani 1 1 d . . . . .
O22 O 0.3142(4) 0.8676(4) -0.0674(4) 0.0111(10) Uani 1 1 d . . . . .
O23 O 0.1380(4) 0.7923(4) 0.0485(4) 0.0129(11) Uani 1 1 d . . . . .
O24 O 0.0837(4) 0.6363(4) 0.2048(4) 0.0118(10) Uani 1 1 d . . . . .
O25 O 0.2785(4) 0.5821(4) 0.0871(4) 0.0107(10) Uani 1 1 d . . . . .
O26 O 0.4596(4) 0.6516(4) -0.0258(4) 0.0124(11) Uani 1 1 d . . . . .
O27 O 0.5732(4) 0.6555(4) 0.1671(4) 0.0112(10) Uani 1 1 d . . . . .
O28 O 0.5252(4) 0.7825(4) 0.2726(4) 0.0131(11) Uani 1 1 d . . . . .
O29 O 0.5827(4) 0.2848(4) 0.3024(4) 0.0132(11) Uani 1 1 d . . . . .
O30 O 0.6959(5) 0.5689(4) 0.3236(4) 0.0151(11) Uani 1 1 d . . . . .
O31 O 0.2776(5) 0.6792(4) 0.5780(4) 0.0148(11) Uani 1 1 d . . . . .
O32 O 0.3982(5) 1.0088(5) 0.2446(4) 0.0177(12) Uani 1 1 d . . . . .
O33 O 0.0206(5) 1.1344(4) 0.1442(4) 0.0145(11) Uani 1 1 d . . . . .
O34 O -0.0885(5) 0.7922(4) 0.4772(4) 0.0155(11) Uani 1 1 d . . . . .
O35 O -0.1012(5) 0.8222(4) 0.1091(4) 0.0156(11) Uani 1 1 d . . . . .
O36 O 0.1726(4) 0.3959(4) 0.5530(4) 0.0131(11) Uani 1 1 d . . . . .
O37 O 0.1648(5) 0.4243(4) 0.1848(4) 0.0139(11) Uani 1 1 d . . . . .
O38 O 0.2671(5) 0.7237(4) -0.1137(4) 0.0153(11) Uani 1 1 d . . . . .
O39 O 0.6880(4) 0.5862(4) 0.0060(4) 0.0135(11) Uani 1 1 d . . . . .
O40 O 0.3858(5) 1.0355(4) -0.0839(4) 0.0152(11) Uani 1 1 d . . . . .
O41 O 0.5827(5) 0.1027(5) 0.5089(4) 0.0179(12) Uani 1 1 d . . . . .
O42 O 0.7985(5) 0.0809(5) 0.3758(5) 0.0225(13) Uani 1 1 d . . . . .
O43 O 0.7142(5) 0.0288(4) 0.2658(4) 0.0191(12) Uani 1 1 d . . . . .
O44 O 0.4924(5) 0.0852(4) 0.3779(4) 0.0165(12) Uani 1 1 d . . . . .
O45 O 0.6762(5) -0.1289(5) 0.4802(4) 0.0201(12) Uani 1 1 d . . . . .
O46 O -0.2062(4) 1.3526(5) 0.2141(4) 0.0163(12) Uani 1 1 d . . . . .
O47 O -0.0866(5) 1.4006(4) 0.0237(4) 0.0143(11) Uani 1 1 d . . . . .
O48 O 0.1249(5) 1.3041(5) 0.1044(4) 0.0221(13) Uani 1 1 d . . . . .
O49 O -0.0076(5) 1.2688(5) 0.2901(4) 0.0198(12) Uani 1 1 d . . . . .
O50 O -0.0711(5) 1.5274(5) 0.1354(4) 0.0175(12) Uani 1 1 d . . . . .
O51W O 0.4162(6) 0.2024(5) 0.2092(4) 0.0304(15) Uani 1 1 d . . . . .
O52W O 0.7682(5) 0.7492(5) 0.0553(4) 0.0197(12) Uani 1 1 d . . . . .
O53W O 0.6891(5) 0.8293(5) 0.3167(4) 0.0215(13) Uani 1 1 d . . . . .
O54W O 0.1161(6) 0.9876(6) 0.4590(6) 0.0413(18) Uani 1 1 d . . . . .
O55W O 0.2049(6) 1.1638(6) 0.3403(5) 0.0437(19) Uani 1 1 d . . . . .
O56W O 0.0641(5) 0.5497(5) 0.6624(4) 0.0246(13) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O1 2.350(5) . ?
W1 O5 1.912(5) . ?
W1 O6 1.908(5) . ?
W1 O7 1.889(5) . ?
W1 O8 1.921(5) . ?
W1 O29 1.720(5) . ?
W2 O1 2.354(5) . ?
W2 O8 1.902(5) . ?
W2 O9 1.910(5) . ?
W2 O10 1.921(5) . ?
W2 O11 1.923(5) . ?
W2 O36 1.703(5) . ?
W3 O2 2.342(5) . ?
W3 O11 1.877(5) . ?
W3 O12 1.904(5) . ?
W3 O13 1.940(5) . ?
W3 O14 1.919(5) . ?
W3 O31 1.707(5) . ?
W4 O2 2.343(5) . ?
W4 O7 1.910(5) . ?
W4 O12 1.914(5) . ?
W4 O27 1.917(5) . ?
W4 O28 1.920(5) . ?
W4 O30 1.706(5) . ?
W5 O3 2.350(5) . ?
W5 O5 1.896(5) . ?
W5 O21 1.943(5) . ?
W5 O26 1.918(5) . ?
W5 O27 1.893(5) . ?
W5 O39 1.702(5) . ?
W6 O1 2.325(5) . ?
W6 O6 1.941(5) . ?
W6 O9 1.931(5) . ?
W6 O24 1.873(5) . ?
W6 O25 1.907(5) . ?
W6 O37 1.704(5) . ?
W7 O3 2.328(5) . ?
W7 O22 1.936(5) . ?
W7 O23 1.913(5) . ?
W7 O25 1.895(5) . ?
W7 O26 1.916(5) . ?
W7 O38 1.705(5) . ?
W8 O3 2.363(5) . ?
W8 O18 1.911(5) . ?
W8 O20 1.908(5) . ?
W8 O21 1.924(5) . ?
W8 O22 1.917(5) . ?
W8 O40 1.701(5) . ?
W9 O4 2.353(5) . ?
W9 O15 1.924(5) . ?
W9 O17 1.895(5) . ?
W9 O23 1.884(5) . ?
W9 O24 1.944(5) . ?
W9 O35 1.703(5) . ?
W10 O4 2.319(5) . ?
W10 O10 1.879(5) . ?
W10 O14 1.907(5) . ?
W10 O15 1.910(5) . ?
W10 O16 1.956(5) . ?
W10 O34 1.710(5) . ?
W11 O2 2.329(5) . ?
W11 O13 1.949(5) . ?
W11 O19 1.907(5) . ?
W11 O20 1.886(5) . ?
W11 O28 1.926(5) . ?
W11 O32 1.696(5) . ?
W12 O4 2.383(5) . ?
W12 O16 1.923(5) . ?
W12 O17 1.924(5) . ?
W12 O18 1.901(5) . ?
W12 O19 1.913(5) . ?
W12 O33 1.704(5) . ?
Cu1 O29 2.413(5) . ?
Cu1 O41 1.996(6) . ?
Cu1 O42 1.949(5) . ?
Cu1 O43 1.978(6) . ?
Cu1 O44 1.962(5) . ?
Cu1 O45 2.524(5) . ?
Cu2 O33 2.596(5) . ?
Cu2 O46 1.956(5) . ?
Cu2 O47 1.972(5) . ?
Cu2 O48 1.960(6) . ?
Cu2 O49 1.950(6) . ?
Cu2 O50 2.473(6) . ?
Si1 O1 1.632(5) . ?
Si1 O2 1.637(5) . ?
Si1 O3 1.625(5) . ?
Si1 O4 1.619(5) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O5 W1 O1 84.91(19) . . ?
O5 W1 O8 158.6(2) . . ?
O6 W1 O1 72.34(19) . . ?
O6 W1 O5 88.4(2) . . ?
O6 W1 O8 87.6(2) . . ?
O7 W1 O1 84.36(19) . . ?
O7 W1 O5 85.5(2) . . ?
O7 W1 O6 156.3(2) . . ?
O7 W1 O8 89.8(2) . . ?
O8 W1 O1 73.89(19) . . ?
O29 W1 O1 169.3(2) . . ?
O29 W1 O5 102.2(2) . . ?
O29 W1 O6 99.6(2) . . ?
O29 W1 O7 104.0(2) . . ?
O29 W1 O8 99.2(2) . . ?
O8 W2 O1 74.11(18) . . ?
O8 W2 O9 89.4(2) . . ?
O8 W2 O10 157.0(2) . . ?
O8 W2 O11 89.8(2) . . ?
O9 W2 O1 73.80(18) . . ?
O9 W2 O10 88.4(2) . . ?
O9 W2 O11 156.6(2) . . ?
O10 W2 O1 83.31(19) . . ?
O10 W2 O11 83.3(2) . . ?
O11 W2 O1 83.54(19) . . ?
O36 W2 O1 172.5(2) . . ?
O36 W2 O8 101.0(2) . . ?
O36 W2 O9 100.7(2) . . ?
O36 W2 O10 101.9(2) . . ?
O36 W2 O11 102.3(2) . . ?
O11 W3 O2 85.0(2) . . ?
O11 W3 O12 90.7(2) . . ?
O11 W3 O13 157.6(2) . . ?
O11 W3 O14 86.0(2) . . ?
O12 W3 O2 73.6(2) . . ?
O12 W3 O13 87.0(2) . . ?
O12 W3 O14 156.6(2) . . ?
O13 W3 O2 72.97(19) . . ?
O14 W3 O2 83.0(2) . . ?
O14 W3 O13 87.3(2) . . ?
O31 W3 O2 170.4(2) . . ?
O31 W3 O11 103.9(2) . . ?
O31 W3 O12 102.6(2) . . ?
O31 W3 O13 98.3(2) . . ?
O31 W3 O14 100.7(2) . . ?
O7 W4 O2 84.11(19) . . ?
O7 W4 O12 89.3(2) . . ?
O7 W4 O27 85.3(2) . . ?
O7 W4 O28 157.2(2) . . ?
O12 W4 O2 73.38(19) . . ?
O12 W4 O27 156.3(2) . . ?
O12 W4 O28 87.8(2) . . ?
O27 W4 O2 83.1(2) . . ?
O27 W4 O28 88.3(2) . . ?
O28 W4 O2 73.38(19) . . ?
O30 W4 O2 171.0(2) . . ?
O30 W4 O7 103.9(2) . . ?
O30 W4 O12 102.3(2) . . ?
O30 W4 O27 101.4(2) . . ?
O30 W4 O28 98.8(2) . . ?
O5 W5 O3 85.04(19) . . ?
O5 W5 O21 157.9(2) . . ?
O5 W5 O26 90.0(2) . . ?
O21 W5 O3 73.06(19) . . ?
O26 W5 O3 73.26(19) . . ?
O26 W5 O21 86.5(2) . . ?
O27 W5 O3 83.53(19) . . ?
O27 W5 O5 86.8(2) . . ?
O27 W5 O21 87.9(2) . . ?
O27 W5 O26 156.8(2) . . ?
O39 W5 O3 171.6(2) . . ?
O39 W5 O5 101.8(2) . . ?
O39 W5 O21 100.2(2) . . ?
O39 W5 O26 101.7(2) . . ?
O39 W5 O27 101.5(2) . . ?
O6 W6 O1 72.37(19) . . ?
O9 W6 O1 74.14(19) . . ?
O9 W6 O6 87.2(2) . . ?
O24 W6 O1 85.48(19) . . ?
O24 W6 O6 157.5(2) . . ?
O24 W6 O9 90.4(2) . . ?
O24 W6 O25 86.9(2) . . ?
O25 W6 O1 85.26(19) . . ?
O25 W6 O6 87.5(2) . . ?
O25 W6 O9 159.4(2) . . ?
O37 W6 O1 169.7(2) . . ?
O37 W6 O6 99.2(2) . . ?
O37 W6 O9 100.0(2) . . ?
O37 W6 O24 103.3(2) . . ?
O37 W6 O25 100.5(2) . . ?
O22 W7 O3 74.10(18) . . ?
O23 W7 O3 84.10(19) . . ?
O23 W7 O22 88.6(2) . . ?
O23 W7 O26 157.8(2) . . ?
O25 W7 O3 84.93(19) . . ?
O25 W7 O22 158.8(2) . . ?
O25 W7 O23 85.8(2) . . ?
O25 W7 O26 89.9(2) . . ?
O26 W7 O3 73.82(19) . . ?
O26 W7 O22 87.5(2) . . ?
O38 W7 O3 170.1(2) . . ?
O38 W7 O22 98.1(2) . . ?
O38 W7 O23 102.1(2) . . ?
O38 W7 O25 103.1(2) . . ?
O38 W7 O26 100.1(2) . . ?
O18 W8 O3 84.59(19) . . ?
O18 W8 O21 157.2(2) . . ?
O18 W8 O22 90.3(2) . . ?
O20 W8 O3 84.06(18) . . ?
O20 W8 O18 84.8(2) . . ?
O20 W8 O21 88.3(2) . . ?
O20 W8 O22 157.5(2) . . ?
O21 W8 O3 73.06(18) . . ?
O22 W8 O3 73.58(18) . . ?
O22 W8 O21 87.8(2) . . ?
O40 W8 O3 171.0(2) . . ?
O40 W8 O18 101.7(2) . . ?
O40 W8 O20 102.8(2) . . ?
O40 W8 O21 101.0(2) . . ?
O40 W8 O22 99.7(2) . . ?
O15 W9 O4 72.60(19) . . ?
O15 W9 O24 86.9(2) . . ?
O17 W9 O4 74.54(19) . . ?
O17 W9 O15 88.4(2) . . ?
O17 W9 O24 157.5(2) . . ?
O23 W9 O4 84.5(2) . . ?
O23 W9 O15 156.2(2) . . ?
O23 W9 O17 91.9(2) . . ?
O23 W9 O24 83.9(2) . . ?
O24 W9 O4 83.03(18) . . ?
O35 W9 O4 171.6(2) . . ?
O35 W9 O15 100.2(2) . . ?
O35 W9 O17 101.3(2) . . ?
O35 W9 O23 103.1(2) . . ?
O35 W9 O24 101.2(2) . . ?
O10 W10 O4 85.7(2) . . ?
O10 W10 O14 86.8(2) . . ?
O10 W10 O15 90.7(2) . . ?
O10 W10 O16 159.2(2) . . ?
O14 W10 O4 83.6(2) . . ?
O14 W10 O15 157.2(2) . . ?
O14 W10 O16 87.2(2) . . ?
O15 W10 O4 73.64(19) . . ?
O15 W10 O16 87.2(2) . . ?
O16 W10 O4 73.78(19) . . ?
O34 W10 O4 171.1(2) . . ?
O34 W10 O10 101.8(2) . . ?
O34 W10 O14 101.3(2) . . ?
O34 W10 O15 101.3(2) . . ?
O34 W10 O16 98.9(2) . . ?
O13 W11 O2 73.13(19) . . ?
O19 W11 O2 85.22(19) . . ?
O19 W11 O13 88.2(2) . . ?
O19 W11 O28 158.8(2) . . ?
O20 W11 O2 85.30(19) . . ?
O20 W11 O13 158.3(2) . . ?
O20 W11 O19 87.3(2) . . ?
O20 W11 O28 90.2(2) . . ?
O28 W11 O2 73.60(19) . . ?
O28 W11 O13 86.4(2) . . ?
O32 W11 O2 168.3(2) . . ?
O32 W11 O13 98.0(2) . . ?
O32 W11 O19 102.5(2) . . ?
O32 W11 O20 103.7(2) . . ?
O32 W11 O28 98.6(2) . . ?
O16 W12 O4 72.83(19) . . ?
O16 W12 O17 87.3(2) . . ?
O17 W12 O4 73.32(18) . . ?
O18 W12 O4 83.60(19) . . ?
O18 W12 O16 156.2(2) . . ?
O18 W12 O17 89.2(2) . . ?
O18 W12 O19 85.7(2) . . ?
O19 W12 O4 83.56(19) . . ?
O19 W12 O16 88.3(2) . . ?
O19 W12 O17 156.7(2) . . ?
O33 W12 O4 170.6(2) . . ?
O33 W12 O16 99.4(2) . . ?
O33 W12 O17 101.5(2) . . ?
O33 W12 O18 104.3(2) . . ?
O33 W12 O19 101.8(2) . . ?
O29 Cu1 O45 169.43(18) . . ?
O41 Cu1 O29 86.6(2) . . ?
O41 Cu1 O45 86.1(2) . . ?
O42 Cu1 O29 87.9(2) . . ?
O42 Cu1 O41 92.6(2) . . ?
O42 Cu1 O43 88.9(3) . . ?
O42 Cu1 O44 177.0(2) . . ?
O42 Cu1 O45 100.0(2) . . ?
O43 Cu1 O29 103.0(2) . . ?
O43 Cu1 O41 170.3(2) . . ?
O43 Cu1 O45 84.3(2) . . ?
O44 Cu1 O29 89.50(19) . . ?
O44 Cu1 O41 88.8(2) . . ?
O44 Cu1 O43 90.3(2) . . ?
O44 Cu1 O45 82.71(19) . . ?
O46 Cu2 O33 98.6(2) . . ?
O46 Cu2 O47 89.0(2) . . ?
O46 Cu2 O48 177.0(2) . . ?
O46 Cu2 O50 91.6(2) . . ?
O47 Cu2 O33 87.15(19) . . ?
O47 Cu2 O50 86.51(19) . . ?
O48 Cu2 O33 80.0(2) . . ?
O48 Cu2 O47 93.6(2) . . ?
O48 Cu2 O50 90.2(2) . . ?
O49 Cu2 O33 94.6(2) . . ?
O49 Cu2 O46 87.8(2) . . ?
O49 Cu2 O47 176.5(2) . . ?
O49 Cu2 O48 89.6(2) . . ?
O49 Cu2 O50 92.3(2) . . ?
O50 Cu2 O33 167.92(18) . . ?
O1 Si1 O2 109.4(3) . . ?
O3 Si1 O1 109.1(3) . . ?
O3 Si1 O2 109.7(3) . . ?
O4 Si1 O1 109.3(3) . . ?
O4 Si1 O2 109.4(3) . . ?
O4 Si1 O3 109.9(3) . . ?
W1 O1 W2 90.40(16) . . ?
W6 O1 W1 92.54(16) . . ?
W6 O1 W2 91.14(16) . . ?
Si1 O1 W1 124.1(3) . . ?
Si1 O1 W2 125.3(3) . . ?
Si1 O1 W6 123.5(3) . . ?
W3 O2 W4 90.96(17) . . ?
W11 O2 W3 92.87(18) . . ?
W11 O2 W4 91.70(17) . . ?
Si1 O2 W3 123.8(3) . . ?
Si1 O2 W4 124.5(3) . . ?
Si1 O2 W11 123.6(3) . . ?
W5 O3 W8 91.76(16) . . ?
W7 O3 W5 91.34(17) . . ?
W7 O3 W8 91.28(16) . . ?
Si1 O3 W5 124.1(3) . . ?
Si1 O3 W7 124.8(3) . . ?
Si1 O3 W8 123.8(3) . . ?
W9 O4 W12 89.86(16) . . ?
W10 O4 W9 91.71(17) . . ?
W10 O4 W12 92.00(17) . . ?
Si1 O4 W9 124.7(3) . . ?
Si1 O4 W10 124.2(3) . . ?
Si1 O4 W12 124.4(3) . . ?
W5 O5 W1 150.9(3) . . ?
W1 O6 W6 122.7(3) . . ?
W1 O7 W4 153.2(3) . . ?
W2 O8 W1 121.6(2) . . ?
W2 O9 W6 120.9(2) . . ?
W10 O10 W2 153.0(3) . . ?
W3 O11 W2 154.3(3) . . ?
W3 O12 W4 122.1(3) . . ?
W3 O13 W11 121.0(3) . . ?
W10 O14 W3 149.8(3) . . ?
W10 O15 W9 122.0(2) . . ?
W12 O16 W10 121.4(3) . . ?
W9 O17 W12 122.3(3) . . ?
W12 O18 W8 153.5(3) . . ?
W11 O19 W12 150.1(3) . . ?
W11 O20 W8 151.7(3) . . ?
W8 O21 W5 122.1(3) . . ?
W8 O22 W7 121.0(2) . . ?
W9 O23 W7 153.8(3) . . ?
W6 O24 W9 151.9(3) . . ?
W7 O25 W6 149.8(3) . . ?
W7 O26 W5 121.6(3) . . ?
W5 O27 W4 151.8(3) . . ?
W4 O28 W11 121.3(3) . . ?
W1 O29 Cu1 148.7(3) . . ?
W12 O33 Cu2 156.4(3) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O1 W1 O7 W4 -58.3(7) . . . . ?
O1 W1 O29 Cu1 -18.7(16) . . . . ?
O1 W6 O24 W9 58.0(6) . . . . ?
O1 Si1 O2 W3 -59.1(4) . . . . ?
O1 Si1 O2 W4 59.8(4) . . . . ?
O1 Si1 O2 W11 179.8(3) . . . . ?
O1 Si1 O3 W5 -60.5(3) . . . . ?
O1 Si1 O3 W7 59.8(4) . . . . ?
O1 Si1 O3 W8 179.7(3) . . . . ?
O1 Si1 O4 W9 -62.1(4) . . . . ?
O1 Si1 O4 W10 58.8(4) . . . . ?
O1 Si1 O4 W12 179.9(3) . . . . ?
O2 W3 O11 W2 -56.3(7) . . . . ?
O2 W11 O20 W8 58.9(6) . . . . ?
O2 Si1 O1 W1 -59.6(4) . . . . ?
O2 Si1 O1 W2 59.7(4) . . . . ?
O2 Si1 O1 W6 179.6(3) . . . . ?
O2 Si1 O3 W5 59.3(4) . . . . ?
O2 Si1 O3 W7 179.6(3) . . . . ?
O2 Si1 O3 W8 -60.5(3) . . . . ?
O2 Si1 O4 W9 178.2(3) . . . . ?
O2 Si1 O4 W10 -61.0(4) . . . . ?
O2 Si1 O4 W12 60.1(4) . . . . ?
O3 W5 O5 W1 -57.5(6) . . . . ?
O3 W5 O27 W4 63.9(6) . . . . ?
O3 W7 O25 W6 57.9(5) . . . . ?
O3 Si1 O1 W1 60.4(4) . . . . ?
O3 Si1 O1 W2 179.7(3) . . . . ?
O3 Si1 O1 W6 -60.4(4) . . . . ?
O3 Si1 O2 W3 -178.8(3) . . . . ?
O3 Si1 O2 W4 -59.8(4) . . . . ?
O3 Si1 O2 W11 60.1(4) . . . . ?
O3 Si1 O4 W9 57.7(4) . . . . ?
O3 Si1 O4 W10 178.6(3) . . . . ?
O3 Si1 O4 W12 -60.3(4) . . . . ?
O4 W9 O17 W12 0.1(3) . . . . ?
O4 W9 O23 W7 55.3(7) . . . . ?
O4 W10 O10 W2 56.0(7) . . . . ?
O4 Si1 O1 W1 -179.4(3) . . . . ?
O4 Si1 O1 W2 -60.1(4) . . . . ?
O4 Si1 O1 W6 59.8(4) . . . . ?
O4 Si1 O2 W3 60.6(4) . . . . ?
O4 Si1 O2 W4 179.6(3) . . . . ?
O4 Si1 O2 W11 -60.5(4) . . . . ?
O4 Si1 O3 W5 179.6(3) . . . . ?
O4 Si1 O3 W7 -60.1(4) . . . . ?
O4 Si1 O3 W8 59.8(4) . . . . ?
O5 W1 O7 W4 27.0(7) . . . . ?
O5 W1 O29 Cu1 -149.4(5) . . . . ?
O5 W5 O27 W4 -21.5(6) . . . . ?
O6 W1 O7 W4 -48.4(10) . . . . ?
O6 W1 O29 Cu1 -59.1(6) . . . . ?
O6 W6 O24 W9 48.4(10) . . . . ?
O7 W1 O29 Cu1 122.2(5) . . . . ?
O8 W1 O7 W4 -132.1(7) . . . . ?
O8 W1 O29 Cu1 30.1(6) . . . . ?
O9 W6 O24 W9 132.1(6) . . . . ?
O12 W3 O11 W2 -129.7(7) . . . . ?
O13 W3 O11 W2 -45.8(11) . . . . ?
O13 W11 O20 W8 51.7(10) . . . . ?
O14 W3 O11 W2 27.1(7) . . . . ?
O14 W10 O10 W2 -27.8(7) . . . . ?
O15 W9 O17 W12 72.5(3) . . . . ?
O15 W9 O23 W7 39.4(10) . . . . ?
O15 W10 O10 W2 129.6(7) . . . . ?
O16 W10 O10 W2 45.7(11) . . . . ?
O16 W12 O33 Cu2 66.4(7) . . . . ?
O17 W9 O23 W7 129.6(7) . . . . ?
O17 W12 O33 Cu2 155.5(7) . . . . ?
O18 W12 O33 Cu2 -112.4(7) . . . . ?
O19 W11 O20 W8 -26.6(6) . . . . ?
O19 W12 O33 Cu2 -23.8(8) . . . . ?
O21 W5 O5 W1 -50.1(9) . . . . ?
O21 W5 O27 W4 137.0(6) . . . . ?
O22 W7 O25 W6 48.6(9) . . . . ?
O23 W7 O25 W6 -26.6(6) . . . . ?
O23 W9 O17 W12 -83.7(3) . . . . ?
O24 W9 O17 W12 -5.4(8) . . . . ?
O24 W9 O23 W7 -28.3(7) . . . . ?
O25 W6 O24 W9 -27.5(6) . . . . ?
O26 W5 O5 W1 -130.7(6) . . . . ?
O26 W5 O27 W4 60.9(9) . . . . ?
O26 W7 O25 W6 131.6(6) . . . . ?
O27 W5 O5 W1 26.3(6) . . . . ?
O28 W11 O20 W8 132.4(6) . . . . ?
O29 W1 O7 W4 128.5(6) . . . . ?
O31 W3 O11 W2 127.1(7) . . . . ?
O32 W11 O20 W8 -128.7(6) . . . . ?
O34 W10 O10 W2 -128.7(7) . . . . ?
O35 W9 O17 W12 172.5(3) . . . . ?
O35 W9 O23 W7 -128.4(7) . . . . ?
O37 W6 O24 W9 -127.6(6) . . . . ?
O38 W7 O25 W6 -128.1(6) . . . . ?
O39 W5 O5 W1 127.4(6) . . . . ?
O39 W5 O27 W4 -122.9(6) . . . . ?

_shelx_SHELXL_version_number     2014/7
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
_exptl_oxdiff_crystal_face_indexfrac_h
_exptl_oxdiff_crystal_face_indexfrac_k
_exptl_oxdiff_crystal_face_indexfrac_l
_exptl_oxdiff_crystal_face_x
_exptl_oxdiff_crystal_face_y
_exptl_oxdiff_crystal_face_z
12 16 18 0.1242 12.0094 15.9766 18.0729 -0.3563 -0.4662 0.8098
-3 -11 -21 0.0570 -3.1513 -10.8198 -20.9961 0.5758 0.7505 -0.3244
-3 6 19 0.0968 -2.7509 5.8307 19.1348 -0.6091 -0.7927 -0.0253
13 18 12 0.1303 13.2373 18.3140 12.3229 -0.3418 -0.1030 0.9341
17 13 6 0.2080 17.3572 12.9022 5.8660 0.1748 0.0496 0.9834
1 -15 -15 0.0342 0.9845 -15.4299 -14.6372 0.9160 0.2714 -0.2954
-2 14 14 0.0955 -2.4565 14.4385 14.2349 -0.9366 -0.2773 0.2143
-16 -16 -9 0.2167 -15.9977 -15.9988 -9.0083 0.0670 0.0122 -0.9962
-7 11 13 0.1033 -7.0201 10.9703 12.9971 -0.9824 -0.3083 -0.0471
-7 10 -7 0.0672 -7.0135 9.9894 -7.0037 -0.7180 0.6858 -0.0075
-16 -2 -11 0.1639 -16.0098 -2.0084 -11.0083 -0.5542 0.5458 -0.6452
8 -9 8 0.0921 8.0132 -8.9899 8.0042 0.7091 -0.7090 0.0684
-1 -16 3 0.0807 -0.9873 -15.9909 2.9996 0.6542 -0.6437 -0.4430
-3 5 19 0.0755 -3.0126 4.9748 18.9993 -0.5808 -0.8114 -0.0563
14 16 16 0.1224 13.9939 15.9899 16.0076 -0.2392 -0.3654 0.8948
-4 11 16 0.0806 -4.0181 10.9713 15.9987 -0.8715 -0.4702 0.0616

_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_cusiw_3_210116_red_075_absent_re
_database_code_depnum_ccdc_archive 'CCDC 1466493'
_audit_update_record             
;
2016-03-14 deposited with the CCDC.
2016-05-19 downloaded from the CCDC.
;
_audit_creation_date             2016-02-03
_audit_creation_method           
;
Olex2 1.2
(compiled 2015.09.30 svn.r3233 for OlexSys, GUI svn.r5103)
;
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Cu2 O50 Si W12, 6(O)'
_chemical_formula_sum            'Cu2 H32 O56 Si W12'
_chemical_formula_weight         3289.62
_chemical_melting_point          ?
_chemical_oxdiff_formula         'Cu2 Si W12 O56 H32'
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/n 1'
_space_group_name_Hall           '-P 2yn'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'

_cell_length_a                   12.9010(3)
_cell_length_b                   22.1952(4)
_cell_length_c                   15.3468(3)
_cell_angle_alpha                90
_cell_angle_beta                 94.432(2)
_cell_angle_gamma                90
_cell_volume                     4381.25(16)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    11581
_cell_measurement_temperature    123.7(6)
_cell_measurement_theta_max      28.7360
_cell_measurement_theta_min      1.8200
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    32.476
_exptl_absorpt_correction_T_max  0.506
_exptl_absorpt_correction_T_min  0.359
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details   
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
Analytical numeric absorption correction using a multifaceted crystal
			model based on expressions derived by R.C. Clark & J.S. Reid.
(Clark, R. C. & Reid, J. S. (1995). Acta Cryst. A51, 887-897)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            'light blue'
_exptl_crystal_colour_modifier   light
_exptl_crystal_colour_primary    blue
_exptl_crystal_density_diffrn    4.987
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       prism
_exptl_crystal_F_000             5760
_exptl_crystal_size_max          0.2192
_exptl_crystal_size_mid          0.1508
_exptl_crystal_size_min          0.1283
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0331
_diffrn_reflns_av_unetI/netI     0.0386
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.993
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       28
_diffrn_reflns_limit_k_min       -28
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            25942
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.993
_diffrn_reflns_theta_full        26.000
_diffrn_reflns_theta_max         27.500
_diffrn_reflns_theta_min         1.830
_diffrn_ambient_environment      N~2~
_diffrn_ambient_temperature      123.7(6)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 16.1183
_diffrn_detector_type            Eos
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_details      
;
#__ type_ start__ end____ width___ exp.time_
  1 omega   26.00   60.00   1.0000   75.3900
omega____ theta____ kappa____ phi______ frames
    -       27.0496  -37.0000  120.0000 34

#__ type_ start__ end____ width___ exp.time_
  2 omega  -11.00   17.00   1.0000   75.3900
omega____ theta____ kappa____ phi______ frames
    -      -27.9089  -88.0000 -145.5107 28

#__ type_ start__ end____ width___ exp.time_
  3 omega  -25.00   52.00   1.0000   75.3900
omega____ theta____ kappa____ phi______ frames
    -      -27.9089   37.0000   90.0000 77

#__ type_ start__ end____ width___ exp.time_
  4 omega  -89.00    6.00   1.0000   75.3900
omega____ theta____ kappa____ phi______ frames
    -      -27.9089  -57.0000  120.0000 95

#__ type_ start__ end____ width___ exp.time_
  5 omega -112.00  -74.00   1.0000   75.3900
omega____ theta____ kappa____ phi______ frames
    -      -27.9089 -178.0000  -30.0000 38

#__ type_ start__ end____ width___ exp.time_
  6 omega -102.00   -1.00   1.0000   75.3900
omega____ theta____ kappa____ phi______ frames
    -      -27.9089  -57.0000  -30.0000 101
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Xcalibur, Eos, Gemini ultra'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_UB_11      -0.0329989000
_diffrn_orient_matrix_UB_12      0.0173601000
_diffrn_orient_matrix_UB_13      0.0249395000
_diffrn_orient_matrix_UB_21      -0.0220772000
_diffrn_orient_matrix_UB_22      -0.0268583000
_diffrn_orient_matrix_UB_23      0.0156379000
_diffrn_orient_matrix_UB_31      0.0382404000
_diffrn_orient_matrix_UB_32      -0.0004131000
_diffrn_orient_matrix_UB_33      0.0357918000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   'Enhance (Mo) X-ray Source'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                8791
_reflns_number_total             9976
_reflns_odcompleteness_completeness 99.98
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     26.32
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_data_collection       
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_data_reduction        
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXS (Sheldrick, 2008)'
_refine_diff_density_max         1.580
_refine_diff_density_min         -1.648
_refine_diff_density_rms         0.295
_refine_ls_extinction_coef       0.000027(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.106
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     641
_refine_ls_number_reflns         9976
_refine_ls_number_restraints     48
_refine_ls_R_factor_all          0.0353
_refine_ls_R_factor_gt           0.0276
_refine_ls_restrained_S_all      1.104
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0179P)²+14.0900P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0553
_refine_ls_wR_factor_ref         0.0575
_refine_special_details          ?
_olex2_refinement_description    
;
1. Uiso/Uaniso restraints and constraints
Uanis(O21) \\sim Ueq, Uanis(O26) \\sim Ueq, Uanis(O19) \\sim Ueq: with sigma of
0.001 and sigma for terminal atoms of 0.001
Uanis(O2) \\sim Ueq, Uanis(O20) \\sim Ueq, Uanis(O42) \\sim Ueq, Uanis(O11)
\\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.005
Uanis(O5) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.01
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W -0.06033(3) 0.83543(2) 0.31103(2) 0.00758(7) Uani 1 1 d . . . . .
W2 W 0.10777(3) 0.71607(2) 0.22926(2) 0.00702(7) Uani 1 1 d . . . . .
W3 W -0.05825(2) 0.61015(2) 0.28684(2) 0.00632(7) Uani 1 1 d . . . . .
W4 W -0.22802(2) 0.72928(2) 0.36715(2) 0.00675(7) Uani 1 1 d . . . . .
W5 W -0.13289(2) 0.82797(2) 0.51763(2) 0.00664(7) Uani 1 1 d . . . . .
W6 W 0.14199(2) 0.82072(2) 0.60215(2) 0.00660(7) Uani 1 1 d . . . . .
W7 W 0.21567(3) 0.82405(2) 0.39487(2) 0.00727(7) Uani 1 1 d . . . . .
W8 W 0.29596(3) 0.71355(2) 0.53347(2) 0.00734(7) Uani 1 1 d . . . . .
W9 W -0.04363(3) 0.70318(2) 0.66286(2) 0.00614(7) Uani 1 1 d . . . . .
W10 W -0.13890(2) 0.60315(2) 0.51161(2) 0.00631(7) Uani 1 1 d . . . . .
W11 W 0.11031(2) 0.59581(2) 0.58898(2) 0.00694(7) Uani 1 1 d . . . . .
W12 W 0.19272(2) 0.60568(2) 0.36483(2) 0.00673(7) Uani 1 1 d . . . . .
Cu1 Cu -0.04718(8) 0.99911(5) 0.16140(7) 0.0123(2) Uani 1 1 d . . . . .
Cu2 Cu -0.12836(8) 0.48016(5) 0.10238(7) 0.0144(2) Uani 1 1 d . . . . .
Si1 Si 0.03377(17) 0.71535(9) 0.44822(13) 0.0040(4) Uani 1 1 d . . . . .
O1 O -0.0620(4) 0.7612(2) 0.4214(3) 0.0066(11) Uani 1 1 d . . . . .
O2 O 0.1359(4) 0.7549(2) 0.4812(3) 0.0054(11) Uani 1 1 d . U . . .
O3 O 0.0600(4) 0.6760(2) 0.3631(3) 0.0057(11) Uani 1 1 d . . . . .
O4 O 0.0028(4) 0.6702(2) 0.5255(3) 0.0068(11) Uani 1 1 d . . . . .
O5 O 0.0760(4) 0.8502(3) 0.3631(4) 0.0106(12) Uani 1 1 d . U . . .
O6 O -0.1154(4) 0.8731(2) 0.4104(3) 0.0087(12) Uani 1 1 d . . . . .
O7 O -0.1890(4) 0.7926(2) 0.2931(3) 0.0093(12) Uani 1 1 d . . . . .
O8 O 0.0040(4) 0.7742(2) 0.2470(3) 0.0077(11) Uani 1 1 d . . . . .
O9 O 0.1958(4) 0.7675(2) 0.3038(3) 0.0097(12) Uani 1 1 d . . . . .
O10 O 0.2046(4) 0.6524(2) 0.2608(4) 0.0096(12) Uani 1 1 d . . . . .
O11 O 0.0056(4) 0.6565(2) 0.2006(3) 0.0078(11) Uani 1 1 d . U . . .
O12 O 0.0700(4) 0.5680(2) 0.3080(3) 0.0099(12) Uani 1 1 d . . . . .
O13 O -0.0918(4) 0.5858(2) 0.4020(3) 0.0074(11) Uani 1 1 d . . . . .
O14 O -0.1552(4) 0.6734(2) 0.3001(3) 0.0089(12) Uani 1 1 d . . . . .
O15 O -0.2479(4) 0.7886(2) 0.4556(3) 0.0089(12) Uani 1 1 d . . . . .
O16 O -0.2096(4) 0.6704(2) 0.4576(3) 0.0070(11) Uani 1 1 d . . . . .
O17 O -0.1460(4) 0.6452(2) 0.6238(3) 0.0089(12) Uani 1 1 d . . . . .
O18 O -0.0234(4) 0.5594(2) 0.5676(3) 0.0077(11) Uani 1 1 d . . . . .
O19 O -0.1211(4) 0.7637(2) 0.5985(3) 0.0075(11) Uani 1 1 d . U . . .
O20 O 0.0695(4) 0.7578(2) 0.6546(3) 0.0063(11) Uani 1 1 d . U . . .
O21 O 0.0540(4) 0.6391(2) 0.6849(3) 0.0062(11) Uani 1 1 d . U . . .
O22 O 0.0084(4) 0.8455(2) 0.5513(3) 0.0087(12) Uani 1 1 d . . . . .
O23 O 0.2038(4) 0.8626(2) 0.5091(3) 0.0084(11) Uani 1 1 d . . . . .
O24 O 0.2671(4) 0.7737(2) 0.6154(3) 0.0086(12) Uani 1 1 d . . . . .
O25 O 0.3247(4) 0.7766(2) 0.4524(4) 0.0106(12) Uani 1 1 d . . . . .
O26 O 0.2706(4) 0.6622(2) 0.4318(3) 0.0088(12) Uani 1 1 d . U . . .
O27 O 0.2144(4) 0.6571(3) 0.5888(3) 0.0097(12) Uani 1 1 d . . . . .
O28 O 0.1409(4) 0.5804(2) 0.4736(3) 0.0074(11) Uani 1 1 d . . . . .
O29 O -0.0774(4) 0.8931(3) 0.2379(3) 0.0115(12) Uani 1 1 d . . . . .
O30 O 0.1431(4) 0.7334(2) 0.1274(3) 0.0097(12) Uani 1 1 d . . . . .
O31 O -0.1264(4) 0.5587(3) 0.2216(3) 0.0105(12) Uani 1 1 d . . . . .
O32 O -0.3547(4) 0.7169(3) 0.3315(4) 0.0128(13) Uani 1 1 d . . . . .
O33 O -0.1957(4) 0.8813(2) 0.5739(3) 0.0117(12) Uani 1 1 d . . . . .
O34 O 0.1624(4) 0.8724(2) 0.6837(3) 0.0094(12) Uani 1 1 d . . . . .
O35 O 0.2877(5) 0.8786(3) 0.3520(4) 0.0133(13) Uani 1 1 d . . . . .
O36 O 0.4209(4) 0.6946(3) 0.5682(4) 0.0129(13) Uani 1 1 d . . . . .
O37 O 0.2820(4) 0.5507(3) 0.3503(4) 0.0133(13) Uani 1 1 d . . . . .
O38 O 0.1732(4) 0.5402(3) 0.6490(4) 0.0123(12) Uani 1 1 d . . . . .
O39 O -0.2366(4) 0.5517(2) 0.5189(4) 0.0098(12) Uani 1 1 d . . . . .
O40 O -0.0760(4) 0.7159(2) 0.7661(3) 0.0099(12) Uani 1 1 d . . . . .
O41 O 0.0192(5) 1.0389(3) 0.2652(4) 0.0181(14) Uani 1 1 d . . . . .
O42 O 0.0837(4) 0.9587(3) 0.1451(4) 0.0169(13) Uani 1 1 d . U . . .
O43 O -0.1208(4) 0.9634(3) 0.0560(4) 0.0135(13) Uani 1 1 d . . . . .
O44 O -0.1757(4) 1.0395(3) 0.1873(4) 0.0142(13) Uani 1 1 d . . . . .
O45 O -0.0010(5) 1.0818(3) 0.0651(4) 0.0152(13) Uani 1 1 d . . . . .
O46 O -0.2777(5) 0.4788(3) 0.1063(4) 0.0186(14) Uani 1 1 d . . . . .
O47 O -0.1230(5) 0.3988(3) 0.1529(4) 0.0175(14) Uani 1 1 d . . . . .
O48 O 0.0239(4) 0.4826(3) 0.1096(4) 0.0150(13) Uani 1 1 d . . . . .
O49 O -0.1334(5) 0.5558(3) 0.0325(4) 0.0149(13) Uani 1 1 d . . . . .
O50 O -0.1099(5) 0.4257(3) -0.0396(4) 0.0193(14) Uani 1 1 d . . . . .
O51W O 0.0898(5) 0.9712(3) 0.4824(5) 0.0267(16) Uani 1 1 d . . . . .
O52W O 0.1269(5) 0.4571(3) 0.2585(4) 0.0170(14) Uani 1 1 d . . . . .
O53W O 0.1099(5) 0.8547(3) 0.0720(4) 0.0207(14) Uani 1 1 d . . . . .
O54W O 0.4514(5) 0.6550(3) 0.2928(4) 0.0239(15) Uani 1 1 d . . . . .
O55W O 0.2027(5) 1.0038(3) 0.3398(4) 0.0268(16) Uani 1 1 d . . . . .
O56W O 0.0326(5) 0.6773(3) -0.0406(4) 0.0187(14) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O1 2.364(5) . ?
W1 O5 1.903(6) . ?
W1 O6 1.923(5) . ?
W1 O7 1.913(6) . ?
W1 O8 1.905(5) . ?
W1 O29 1.705(5) . ?
W2 O3 2.364(5) . ?
W2 O8 1.893(5) . ?
W2 O9 1.923(5) . ?
W2 O10 1.923(6) . ?
W2 O11 1.894(5) . ?
W2 O30 1.706(5) . ?
W3 O3 2.356(5) . ?
W3 O11 1.912(5) . ?
W3 O12 1.907(6) . ?
W3 O13 1.929(5) . ?
W3 O14 1.902(5) . ?
W3 O31 1.716(5) . ?
W4 O1 2.347(5) . ?
W4 O7 1.900(6) . ?
W4 O14 1.905(6) . ?
W4 O15 1.922(6) . ?
W4 O16 1.909(5) . ?
W4 O32 1.705(6) . ?
W5 O1 2.328(5) . ?
W5 O6 1.954(5) . ?
W5 O15 1.911(5) . ?
W5 O19 1.890(5) . ?
W5 O22 1.897(6) . ?
W5 O33 1.706(6) . ?
W6 O2 2.359(5) . ?
W6 O20 1.895(5) . ?
W6 O22 1.916(5) . ?
W6 O23 1.927(5) . ?
W6 O24 1.920(5) . ?
W6 O34 1.703(5) . ?
W7 O2 2.320(5) . ?
W7 O5 1.920(6) . ?
W7 O9 1.882(5) . ?
W7 O23 1.968(5) . ?
W7 O25 1.917(5) . ?
W7 O35 1.691(6) . ?
W8 O2 2.344(5) . ?
W8 O24 1.890(5) . ?
W8 O25 1.928(6) . ?
W8 O26 1.939(5) . ?
W8 O27 1.881(6) . ?
W8 O36 1.711(6) . ?
W9 O4 2.352(5) . ?
W9 O17 1.907(5) . ?
W9 O19 1.904(5) . ?
W9 O20 1.908(5) . ?
W9 O21 1.913(5) . ?
W9 O40 1.693(5) . ?
W10 O4 2.354(5) . ?
W10 O13 1.872(5) . ?
W10 O16 1.904(5) . ?
W10 O17 1.966(5) . ?
W10 O18 1.925(5) . ?
W10 O39 1.711(5) . ?
W11 O4 2.322(5) . ?
W11 O18 1.909(5) . ?
W11 O21 1.945(5) . ?
W11 O27 1.911(6) . ?
W11 O28 1.875(5) . ?
W11 O38 1.708(6) . ?
W12 O3 2.315(5) . ?
W12 O10 1.919(6) . ?
W12 O12 1.937(5) . ?
W12 O26 1.866(5) . ?
W12 O28 1.930(5) . ?
W12 O37 1.705(6) . ?
Cu1 O29 2.672(6) . ?
Cu1 O41 1.960(6) . ?
Cu1 O42 1.944(6) . ?
Cu1 O43 1.978(6) . ?
Cu1 O44 1.953(6) . ?
Cu1 O45 2.458(6) . ?
Cu2 O31 2.526(5) . ?
Cu2 O46 1.933(6) . ?
Cu2 O47 1.965(6) . ?
Cu2 O48 1.960(6) . ?
Cu2 O49 1.991(6) . ?
Cu2 O50 2.519(6) . ?
Si1 O1 1.629(5) . ?
Si1 O2 1.631(5) . ?
Si1 O3 1.629(5) . ?
Si1 O4 1.626(6) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O5 W1 O1 83.0(2) . . ?
O5 W1 O6 88.7(2) . . ?
O5 W1 O7 155.4(2) . . ?
O5 W1 O8 85.1(2) . . ?
O6 W1 O1 73.1(2) . . ?
O7 W1 O1 72.6(2) . . ?
O7 W1 O6 87.7(2) . . ?
O8 W1 O1 84.3(2) . . ?
O8 W1 O6 157.2(2) . . ?
O8 W1 O7 88.8(2) . . ?
O29 W1 O1 170.6(2) . . ?
O29 W1 O5 102.4(3) . . ?
O29 W1 O6 99.2(2) . . ?
O29 W1 O7 102.2(2) . . ?
O29 W1 O8 103.6(2) . . ?
O8 W2 O3 84.1(2) . . ?
O8 W2 O9 84.4(2) . . ?
O8 W2 O10 156.5(2) . . ?
O8 W2 O11 91.2(2) . . ?
O9 W2 O3 83.6(2) . . ?
O9 W2 O10 86.8(2) . . ?
O10 W2 O3 73.3(2) . . ?
O11 W2 O3 73.4(2) . . ?
O11 W2 O9 157.0(2) . . ?
O11 W2 O10 88.4(2) . . ?
O30 W2 O3 170.9(2) . . ?
O30 W2 O8 102.7(2) . . ?
O30 W2 O9 102.9(2) . . ?
O30 W2 O10 100.5(2) . . ?
O30 W2 O11 100.1(2) . . ?
O11 W3 O3 73.3(2) . . ?
O11 W3 O13 157.5(2) . . ?
O12 W3 O3 72.5(2) . . ?
O12 W3 O11 88.1(2) . . ?
O12 W3 O13 87.7(2) . . ?
O13 W3 O3 84.3(2) . . ?
O14 W3 O3 84.0(2) . . ?
O14 W3 O11 89.9(2) . . ?
O14 W3 O12 156.0(2) . . ?
O14 W3 O13 85.0(2) . . ?
O31 W3 O3 170.1(2) . . ?
O31 W3 O11 100.6(2) . . ?
O31 W3 O12 99.9(2) . . ?
O31 W3 O13 101.9(2) . . ?
O31 W3 O14 104.0(2) . . ?
O7 W4 O1 73.3(2) . . ?
O7 W4 O14 89.7(2) . . ?
O7 W4 O15 88.4(2) . . ?
O7 W4 O16 156.6(2) . . ?
O14 W4 O1 85.0(2) . . ?
O14 W4 O15 157.7(2) . . ?
O14 W4 O16 84.7(2) . . ?
O15 W4 O1 73.2(2) . . ?
O16 W4 O1 83.7(2) . . ?
O16 W4 O15 88.3(2) . . ?
O32 W4 O1 171.3(2) . . ?
O32 W4 O7 102.7(3) . . ?
O32 W4 O14 102.8(3) . . ?
O32 W4 O15 99.2(3) . . ?
O32 W4 O16 100.7(2) . . ?
O6 W5 O1 73.5(2) . . ?
O15 W5 O1 73.8(2) . . ?
O15 W5 O6 87.2(2) . . ?
O19 W5 O1 85.4(2) . . ?
O19 W5 O6 158.6(2) . . ?
O19 W5 O15 90.1(2) . . ?
O19 W5 O22 87.1(2) . . ?
O22 W5 O1 83.5(2) . . ?
O22 W5 O6 87.3(2) . . ?
O22 W5 O15 157.3(2) . . ?
O33 W5 O1 171.0(2) . . ?
O33 W5 O6 99.3(2) . . ?
O33 W5 O15 100.9(3) . . ?
O33 W5 O19 102.0(2) . . ?
O33 W5 O22 101.7(2) . . ?
O20 W6 O2 83.7(2) . . ?
O20 W6 O22 85.8(2) . . ?
O20 W6 O23 156.4(2) . . ?
O20 W6 O24 89.6(2) . . ?
O22 W6 O2 83.3(2) . . ?
O22 W6 O23 88.3(2) . . ?
O22 W6 O24 157.1(2) . . ?
O23 W6 O2 72.9(2) . . ?
O24 W6 O2 73.9(2) . . ?
O24 W6 O23 87.0(2) . . ?
O34 W6 O2 171.6(2) . . ?
O34 W6 O20 103.8(2) . . ?
O34 W6 O22 100.8(2) . . ?
O34 W6 O23 99.8(2) . . ?
O34 W6 O24 102.0(2) . . ?
O5 W7 O2 84.0(2) . . ?
O5 W7 O23 87.6(2) . . ?
O9 W7 O2 86.6(2) . . ?
O9 W7 O5 86.7(2) . . ?
O9 W7 O23 159.5(2) . . ?
O9 W7 O25 91.6(2) . . ?
O23 W7 O2 73.2(2) . . ?
O25 W7 O2 73.5(2) . . ?
O25 W7 O5 157.5(2) . . ?
O25 W7 O23 86.2(2) . . ?
O35 W7 O2 167.9(2) . . ?
O35 W7 O5 102.6(3) . . ?
O35 W7 O9 103.7(3) . . ?
O35 W7 O23 96.8(2) . . ?
O35 W7 O25 99.6(3) . . ?
O24 W8 O2 74.8(2) . . ?
O24 W8 O25 88.6(2) . . ?
O24 W8 O26 157.0(2) . . ?
O25 W8 O2 72.7(2) . . ?
O25 W8 O26 86.3(2) . . ?
O26 W8 O2 82.3(2) . . ?
O27 W8 O2 84.6(2) . . ?
O27 W8 O24 91.4(2) . . ?
O27 W8 O25 156.6(2) . . ?
O27 W8 O26 84.6(2) . . ?
O36 W8 O2 170.7(2) . . ?
O36 W8 O24 101.3(3) . . ?
O36 W8 O25 99.0(3) . . ?
O36 W8 O26 101.7(2) . . ?
O36 W8 O27 104.0(3) . . ?
O17 W9 O4 74.1(2) . . ?
O17 W9 O20 157.2(2) . . ?
O17 W9 O21 89.1(2) . . ?
O19 W9 O4 85.1(2) . . ?
O19 W9 O17 89.4(2) . . ?
O19 W9 O20 83.7(2) . . ?
O19 W9 O21 158.2(2) . . ?
O20 W9 O4 83.6(2) . . ?
O20 W9 O21 89.3(2) . . ?
O21 W9 O4 73.6(2) . . ?
O40 W9 O4 171.4(2) . . ?
O40 W9 O17 101.1(2) . . ?
O40 W9 O19 102.2(2) . . ?
O40 W9 O20 101.6(2) . . ?
O40 W9 O21 99.5(2) . . ?
O13 W10 O4 84.7(2) . . ?
O13 W10 O16 87.0(2) . . ?
O13 W10 O17 157.6(2) . . ?
O13 W10 O18 90.2(2) . . ?
O16 W10 O4 83.5(2) . . ?
O16 W10 O17 87.5(2) . . ?
O16 W10 O18 156.6(2) . . ?
O17 W10 O4 73.1(2) . . ?
O18 W10 O4 73.1(2) . . ?
O18 W10 O17 86.3(2) . . ?
O39 W10 O4 170.7(2) . . ?
O39 W10 O13 102.3(2) . . ?
O39 W10 O16 102.8(2) . . ?
O39 W10 O17 100.1(2) . . ?
O39 W10 O18 100.5(2) . . ?
O18 W11 O4 74.1(2) . . ?
O18 W11 O21 87.3(2) . . ?
O18 W11 O27 157.8(2) . . ?
O21 W11 O4 73.7(2) . . ?
O27 W11 O4 83.7(2) . . ?
O27 W11 O21 87.3(2) . . ?
O28 W11 O4 84.1(2) . . ?
O28 W11 O18 90.8(2) . . ?
O28 W11 O21 157.4(2) . . ?
O28 W11 O27 86.0(2) . . ?
O38 W11 O4 169.8(2) . . ?
O38 W11 O18 99.9(2) . . ?
O38 W11 O21 97.9(2) . . ?
O38 W11 O27 102.2(2) . . ?
O38 W11 O28 104.6(2) . . ?
O10 W12 O3 74.5(2) . . ?
O10 W12 O12 88.5(2) . . ?
O10 W12 O28 158.8(2) . . ?
O12 W12 O3 73.0(2) . . ?
O26 W12 O3 85.4(2) . . ?
O26 W12 O10 91.2(2) . . ?
O26 W12 O12 157.7(2) . . ?
O26 W12 O28 85.8(2) . . ?
O28 W12 O3 84.3(2) . . ?
O28 W12 O12 86.5(2) . . ?
O37 W12 O3 171.0(2) . . ?
O37 W12 O10 100.4(3) . . ?
O37 W12 O12 99.7(3) . . ?
O37 W12 O26 102.3(3) . . ?
O37 W12 O28 100.8(3) . . ?
O41 Cu1 O29 96.3(2) . . ?
O41 Cu1 O43 176.2(3) . . ?
O41 Cu1 O45 92.3(2) . . ?
O42 Cu1 O29 79.0(2) . . ?
O42 Cu1 O41 89.0(3) . . ?
O42 Cu1 O43 94.4(2) . . ?
O42 Cu1 O44 175.7(3) . . ?
O42 Cu1 O45 90.8(2) . . ?
O43 Cu1 O29 85.9(2) . . ?
O43 Cu1 O45 86.1(2) . . ?
O44 Cu1 O29 99.2(2) . . ?
O44 Cu1 O41 87.3(2) . . ?
O44 Cu1 O43 89.4(2) . . ?
O44 Cu1 O45 91.6(2) . . ?
O45 Cu1 O29 166.45(18) . . ?
O46 Cu2 O31 86.7(2) . . ?
O46 Cu2 O47 88.7(3) . . ?
O46 Cu2 O48 174.9(3) . . ?
O46 Cu2 O49 92.2(3) . . ?
O46 Cu2 O50 100.4(2) . . ?
O47 Cu2 O31 110.5(2) . . ?
O47 Cu2 O49 170.6(2) . . ?
O47 Cu2 O50 84.1(2) . . ?
O48 Cu2 O31 89.2(2) . . ?
O48 Cu2 O47 89.9(3) . . ?
O48 Cu2 O49 89.9(2) . . ?
O48 Cu2 O50 84.3(2) . . ?
O49 Cu2 O31 78.8(2) . . ?
O49 Cu2 O50 86.6(2) . . ?
O50 Cu2 O31 164.1(2) . . ?
O1 Si1 O2 108.7(3) . . ?
O1 Si1 O3 109.5(3) . . ?
O3 Si1 O2 108.9(3) . . ?
O4 Si1 O1 110.2(3) . . ?
O4 Si1 O2 110.1(3) . . ?
O4 Si1 O3 109.4(3) . . ?
W4 O1 W1 90.83(17) . . ?
W5 O1 W1 92.11(18) . . ?
W5 O1 W4 91.40(18) . . ?
Si1 O1 W1 124.6(3) . . ?
Si1 O1 W4 123.7(3) . . ?
Si1 O1 W5 124.4(3) . . ?
W7 O2 W6 92.87(18) . . ?
W7 O2 W8 92.10(18) . . ?
W8 O2 W6 89.89(18) . . ?
Si1 O2 W6 123.7(3) . . ?
Si1 O2 W7 124.2(3) . . ?
Si1 O2 W8 124.4(3) . . ?
W3 O3 W2 90.25(17) . . ?
W12 O3 W2 91.23(18) . . ?
W12 O3 W3 92.18(18) . . ?
Si1 O3 W2 125.4(3) . . ?
Si1 O3 W3 124.4(3) . . ?
Si1 O3 W12 123.5(3) . . ?
W9 O4 W10 91.62(19) . . ?
W11 O4 W9 91.76(18) . . ?
W11 O4 W10 91.30(19) . . ?
Si1 O4 W9 123.8(3) . . ?
Si1 O4 W10 123.8(3) . . ?
Si1 O4 W11 124.9(3) . . ?
W1 O5 W7 150.8(3) . . ?
W1 O6 W5 121.3(3) . . ?
W4 O7 W1 123.3(3) . . ?
W2 O8 W1 154.3(3) . . ?
W7 O9 W2 151.4(3) . . ?
W12 O10 W2 121.0(3) . . ?
W2 O11 W3 123.0(3) . . ?
W3 O12 W12 122.2(3) . . ?
W10 O13 W3 151.3(3) . . ?
W3 O14 W4 153.5(3) . . ?
W5 O15 W4 121.6(3) . . ?
W10 O16 W4 151.9(3) . . ?
W9 O17 W10 121.2(3) . . ?
W11 O18 W10 121.4(3) . . ?
W5 O19 W9 152.3(3) . . ?
W6 O20 W9 154.4(3) . . ?
W9 O21 W11 120.8(3) . . ?
W5 O22 W6 150.1(3) . . ?
W6 O23 W7 121.0(3) . . ?
W8 O24 W6 121.4(3) . . ?
W7 O25 W8 121.6(3) . . ?
W12 O26 W8 152.7(3) . . ?
W8 O27 W11 153.2(3) . . ?
W11 O28 W12 151.2(3) . . ?
W1 O29 Cu1 159.1(3) . . ?
W3 O31 Cu2 149.1(3) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O1 W5 O19 W9 55.0(6) . . . . ?
O1 W5 O22 W6 -64.7(6) . . . . ?
O1 Si1 O2 W6 60.5(4) . . . . ?
O1 Si1 O2 W7 -61.2(4) . . . . ?
O1 Si1 O2 W8 177.5(3) . . . . ?
O1 Si1 O3 W2 58.3(4) . . . . ?
O1 Si1 O3 W3 -61.2(4) . . . . ?
O1 Si1 O3 W12 178.3(3) . . . . ?
O1 Si1 O4 W9 -59.1(4) . . . . ?
O1 Si1 O4 W10 60.2(4) . . . . ?
O1 Si1 O4 W11 -179.8(3) . . . . ?
O2 W6 O20 W9 -59.1(7) . . . . ?
O2 W7 O9 W2 55.7(6) . . . . ?
O2 W8 O24 W6 0.6(3) . . . . ?
O2 W8 O27 W11 58.0(7) . . . . ?
O2 Si1 O1 W1 60.3(4) . . . . ?
O2 Si1 O1 W4 179.0(3) . . . . ?
O2 Si1 O1 W5 -61.5(4) . . . . ?
O2 Si1 O3 W2 -60.5(4) . . . . ?
O2 Si1 O3 W3 -179.9(3) . . . . ?
O2 Si1 O3 W12 59.6(4) . . . . ?
O2 Si1 O4 W9 60.8(4) . . . . ?
O2 Si1 O4 W10 -179.9(3) . . . . ?
O2 Si1 O4 W11 -60.0(4) . . . . ?
O3 W2 O8 W1 56.2(7) . . . . ?
O3 W2 O11 W3 -0.3(3) . . . . ?
O3 W12 O26 W8 58.8(7) . . . . ?
O3 Si1 O1 W1 -58.6(4) . . . . ?
O3 Si1 O1 W4 60.1(4) . . . . ?
O3 Si1 O1 W5 179.6(3) . . . . ?
O3 Si1 O2 W6 179.8(3) . . . . ?
O3 Si1 O2 W7 58.0(4) . . . . ?
O3 Si1 O2 W8 -63.3(4) . . . . ?
O3 Si1 O4 W9 -179.5(3) . . . . ?
O3 Si1 O4 W10 -60.2(4) . . . . ?
O3 Si1 O4 W11 59.7(4) . . . . ?
O4 W10 O13 W3 -59.8(6) . . . . ?
O4 W11 O28 W12 59.4(6) . . . . ?
O4 Si1 O1 W1 -179.0(3) . . . . ?
O4 Si1 O1 W4 -60.3(4) . . . . ?
O4 Si1 O1 W5 59.2(4) . . . . ?
O4 Si1 O2 W6 -60.3(4) . . . . ?
O4 Si1 O2 W7 178.0(3) . . . . ?
O4 Si1 O2 W8 56.7(4) . . . . ?
O4 Si1 O3 W2 179.1(3) . . . . ?
O4 Si1 O3 W3 59.7(4) . . . . ?
O4 Si1 O3 W12 -60.8(4) . . . . ?
O5 W1 O29 Cu1 -18.5(9) . . . . ?
O5 W7 O9 W2 -28.5(6) . . . . ?
O6 W1 O29 Cu1 72.2(9) . . . . ?
O6 W5 O19 W9 46.2(10) . . . . ?
O6 W5 O22 W6 -138.3(6) . . . . ?
O7 W1 O29 Cu1 161.9(8) . . . . ?
O8 W1 O29 Cu1 -106.4(8) . . . . ?
O8 W2 O11 W3 -83.7(3) . . . . ?
O9 W2 O8 W1 -27.9(7) . . . . ?
O9 W2 O11 W3 -5.2(8) . . . . ?
O10 W2 O8 W1 40.5(11) . . . . ?
O10 W2 O11 W3 72.7(3) . . . . ?
O10 W12 O26 W8 133.1(7) . . . . ?
O11 W2 O8 W1 129.4(7) . . . . ?
O11 W3 O31 Cu2 52.6(6) . . . . ?
O12 W3 O31 Cu2 -37.4(6) . . . . ?
O12 W12 O26 W8 44.2(11) . . . . ?
O13 W3 O31 Cu2 -127.1(6) . . . . ?
O14 W3 O31 Cu2 145.2(5) . . . . ?
O15 W5 O19 W9 128.7(7) . . . . ?
O15 W5 O22 W6 -62.2(9) . . . . ?
O16 W10 O13 W3 23.9(6) . . . . ?
O17 W10 O13 W3 -52.2(10) . . . . ?
O18 W10 O13 W3 -132.8(6) . . . . ?
O18 W11 O28 W12 133.4(6) . . . . ?
O19 W5 O22 W6 21.1(6) . . . . ?
O21 W11 O28 W12 48.4(10) . . . . ?
O22 W5 O19 W9 -28.7(7) . . . . ?
O22 W6 O20 W9 24.7(7) . . . . ?
O23 W6 O20 W9 -51.3(10) . . . . ?
O23 W7 O9 W2 45.6(11) . . . . ?
O24 W6 O20 W9 -132.9(7) . . . . ?
O24 W8 O27 W11 132.6(7) . . . . ?
O25 W7 O9 W2 129.1(7) . . . . ?
O25 W8 O24 W6 73.1(3) . . . . ?
O25 W8 O27 W11 43.0(11) . . . . ?
O26 W8 O24 W6 -4.0(8) . . . . ?
O26 W8 O27 W11 -24.7(7) . . . . ?
O27 W8 O24 W6 -83.5(3) . . . . ?
O27 W11 O28 W12 -24.6(6) . . . . ?
O28 W12 O26 W8 -25.8(7) . . . . ?
O30 W2 O8 W1 -130.0(7) . . . . ?
O30 W2 O11 W3 173.1(3) . . . . ?
O33 W5 O19 W9 -130.1(6) . . . . ?
O33 W5 O22 W6 122.8(6) . . . . ?
O34 W6 O20 W9 124.8(7) . . . . ?
O35 W7 O9 W2 -130.6(6) . . . . ?
O36 W8 O24 W6 172.0(3) . . . . ?
O36 W8 O27 W11 -125.4(7) . . . . ?
O37 W12 O26 W8 -126.0(7) . . . . ?
O38 W11 O28 W12 -126.2(6) . . . . ?
O39 W10 O13 W3 126.3(6) . . . . ?

_shelx_SHELXL_version_number     2014/7
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
_exptl_oxdiff_crystal_face_indexfrac_h
_exptl_oxdiff_crystal_face_indexfrac_k
_exptl_oxdiff_crystal_face_indexfrac_l
_exptl_oxdiff_crystal_face_x
_exptl_oxdiff_crystal_face_y
_exptl_oxdiff_crystal_face_z
15 8 10 0.1115 14.6996 8.3369 9.9563 -0.0920 -0.3927 0.9150
11 -1 16 0.1115 11.4387 -0.5578 15.7104 0.0047 0.0081 1.0000
-6 -21 15 0.0601 -6.4784 -20.6692 14.8201 0.2246 0.9299 0.2912
-14 -19 2 0.0498 -14.4855 -18.8217 2.1760 0.2055 0.8593 -0.4683
-10 4 -17 0.1078 -9.7265 3.8191 -17.1391 -0.0402 -0.1559 -0.9870
2 -31 2 0.0679 1.8056 -31.0218 1.5118 -0.5604 0.8170 0.1360
-9 -19 -12 0.0512 -8.7625 -19.4636 -12.4848 -0.3601 0.5210 -0.7739
-9 20 13 0.0559 -9.0229 19.9001 13.0054 0.9676 -0.1319 0.1122
14 -19 -4 0.0653 14.0109 -18.9226 -4.0099 -0.8908 0.1362 0.4001
-1 -14 -19 0.0638 -0.9706 -13.9117 -18.9983 -0.6833 0.0980 -0.7114
17 -6 -7 0.0646 16.9988 -5.9161 -6.9963 -0.8381 -0.3258 0.4021
4 -4 -21 0.0806 4.0179 -3.9001 -20.9875 -0.7237 -0.3122 -0.5959
17 9 -6 0.0711 16.9838 9.0635 -5.9845 -0.5524 -0.7120 0.4315
2 8 -21 0.0882 2.0080 8.0810 -20.9779 -0.4492 -0.5894 -0.6774
12 23 -5 0.0705 11.9734 23.0297 -4.9747 -0.1194 -0.9607 0.2703
0 19 -17 0.0915 -0.0042 19.0472 -16.9721 -0.0925 -0.7769 -0.6155
-1 31 2 0.0558 -1.0303 30.9552 2.0242 0.6219 -0.7770 0.0203
-5 28 8 0.0509 -5.0294 27.9229 8.0165 0.8506 -0.5136 0.0831
-12 -1 18 0.0601 -12.0048 -1.1057 17.9837 0.8255 0.5760 0.1851

_olex2_submission_special_instructions 'No special instructions were received'
